Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process

*Amaya Igartua, Raquel Bayon, Ana Aranzabe and Javier Laucirica*

### **Abstract**

This chapter describes a summary of the main tribological achievements carried out in TEKNIKER during the last 37 years. It covers the description of commercial and newly developed tribological test benches and case studies for a wide variety of applications. The examples refer to different tribological characterization tools for material selection (e.g., composition, surface treatments, lubricants). It makes emphasis in the failure mechanisms (pitting, scuffing, abrasion, adhesion, thermal fatigue, tribocorrosion, etc.) and friction simulation of a wide range of materials (seals, textiles, steels, cast iron, light alloys, ceramic, composites), tribological systems (mechanical components, biomaterials, tribolubrication), and environments (vacuum, ultrahigh vacuum, low or high temperature, and corrosive). A huge range of new testing equipment and protocols have been developed to simulate the mentioned failure mechanisms and working environments. This knowledge will make possible, in the future, to simulate at laboratory a still wider list of tribological systems and develop new standards. Tribology will help to implement materials solutions into energy and resource efficient products and process, to reduce carbon footprint.

**Keywords:** tribology, tribocorrosion, lubricants, materials, pitting, scuffing, abrasion, adhesion, erosion, thermal fatigue, die soldering, vacuum, ultrahigh vacuum, tribodesorption, outgassing, high temperature, corrosive

### **1. Introduction**

TEKNIKER is a nonprofit applied research institution located in the armoring city of Eibar specialized in manufacturing, precision engineering, and tribology, with a history of 37 years. It is a founded member of the IK4 Research Alliance, a private alliance of seven R&D centers with 1158 persons and 308 PHD, with the mission to generate, capture, and transfer scientific and technological knowledge to industries. The tribology unit from TEKNIKER is working on failure diagnosis, surface characterization, and solving tribological problems in direct collaboration with other units from TEKNIKER like surface physics and chemistry, lubricant chemistry, laser, additive and micro-nano manufacturing, maintenance, mechanical design, sensors, and robotics. TEKNIKER is a European referent in the field of tribology with participation in more than 130 projects (EU, Spanish, and regional) with more than 250 scientific contributions in congresses, journals, and books and 3 patents. It has been active in **several international working groups** and associations, in some of them, acting as Spanish representative:


**149**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

• The Basque Country representation in the materials for batteries S3P Smart

The philosophy from TEKNIKER has been to buy commercial equipment when available and to develop and construct new testing benches, when they are not easily available. Thus, TEKNIKER is equipped with the **most advanced commercial** 

• FALEX **high-performance** and FALEX multispecimen test machines (ASTM

• FALEX **Four-Ball** Machine to measure antiwear properties (ASTM D 2266 for greases, ASTM D 4172 for oils) and extreme pressure properties (ASTM D

• OPTIMOL **SRV-III machine** to measure antiwear properties (ASTM D 5707 for greases, ASTM D 6425 and DIN 51834 for lubricants) and extreme pressure

• CETR UMT-3 **reciprocal tribological test**, Block on Ring Test (ASTM G77), scratch test (ASTM D7027, ASTM G171, ISO 20502), Ball on Flat (ASTM G-133), Friction dissipation (ASTM G-203), Pin Abrasion (ASTM G132), Pin on Disc (ASTM G99), Scratch hardness (ASTM G171), Thrust washer (ASTM D3702), Rolled web friction (ASTM G143), Viscoelastic properties (DIN 53513), Indentation hardness (ISO 14577), Adhesion and mechanical failures

properties (ASTM D 5706 for greases, ASTM D 74121 for lubricants)

• **Twin disc** machine with Block on Ring configuration (e.g., ASTM G176,

• STRAMA FZG **gear test machine**, wear (ASTM D 4998), Micropitting (FVA 54/I-IV), DGMK 575), Pitting (FVA 2/V), Scuffing (DIN 51354-1/2, ISO 14635-1, CEC-L-07-96, IP 334/93, ASTM D5182-91), grease (DIN 74), Extreme

• **Two bearing tests** by Elgeti Engineering to characterize bearings lubricated with greases and oils (DIN51819) and to develop new lubricants, coatings,

rolling bearings designs, and predictive maintenance activities

G99, ASTM D3702, ASTM D5183, ASTM D2266, ASTM D4172)

2596 for greases, ASTM D 2783 and ASTM D-7421 for lubricants)

TEKNIKER has been active in the **organization of Congress** (LUBMAT, IBERTRIB, COST 516, COST 532, COMADEM, EUMAT, NANOFILMS); international meetings in cooperation with MATERPLAT, EMRS, FEMS-SOCIEMAT, EMCC, and EPPN; and **courses** such Marie Curie (Oct. 2011), LUBMAT (2012,

• The European Pilot Projects Network (EPPN) (2017–now)

**equipment** covering a huge range of testing standards such as:

• FALEX **tapping torque test machines** (ASTM D5619)

• CSM **nanotribometer** (Load from 20μN-2N)

Specialization Region initiative (2018–now)

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

2016, 2018), or Erasmus+ (2018).

**2. Commercial equipment**

(ASTM C 1640)

ASTM G77)

Pressure test (FVA 243)

• The materials for construction team of the ECTP Construction Platform (2018–now)

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*


TEKNIKER has been active in the **organization of Congress** (LUBMAT, IBERTRIB, COST 516, COST 532, COMADEM, EUMAT, NANOFILMS); international meetings in cooperation with MATERPLAT, EMRS, FEMS-SOCIEMAT, EMCC, and EPPN; and **courses** such Marie Curie (Oct. 2011), LUBMAT (2012, 2016, 2018), or Erasmus+ (2018).

### **2. Commercial equipment**

*Friction, Lubrication and Wear*

(2002–2007)

(2005–2016)

(2012–now))

(2016–now)

(2016–now)

(2018–now)

with more than 250 scientific contributions in congresses, journals, and books and 3 patents. It has been active in **several international working groups** and associa-

• The COST 532 about tribotechnology of engines and transmissions

• The Virtual Tribology Institute (VTI) involving 22 centers of tribology

• The steering committee member (2005–now) of the European Materials

• The E!-ENIWEP, the Eureka Network for wear prevention (2006–2010)

• The steering committee of EMIRI, the materials for Low Carbon Energy

• The Austrian COMET Action X-Tribology (Excellence Center for Tribology

• The Knowledge-based Multifunctional Materials Virtual Institute (KMM-VIN)

• The CAPTECH Materials for Defense of the European Defence Agency (EDA)

• The Coordination and Support Action (CSA) MATCH, Materials Open House (2014–2017), promoted by the Alliance of Materials A4M that was created by

• The European Materials Modeling and European Materials Characterization

• The materials for construction team of the ECTP Construction Platform

• The NANOMAT (Basque materials and nanotechnologies team (2005–2006))

Platform (EuMaT) holding since 2017 the co-secretary

• The MATERPLAT Spanish Materials Platform (2009–now)

• The E!-SURF, the Eureka Umbrella on Surfaces (2010–2016)

• The Network 2B Funtex on Functional Textiles (2011–2014)

• The International Tribology Council (2014–now)

• The BIC, Biobased Industries Consortium (2014–now)

• The ECP4 Network about plastics and composites (2015–now)

Suschem, Nanofuture, EMRS, FEMS, EMIRI, and EUMAT

Councils (EMMC-EMCC) (2017–now)

Industrial Initiative (2012–now)

tions, in some of them, acting as Spanish representative:

• The COST 516 about tribology (1995–2000)

• The COST 533 on biotribology (2003–2008)

**148**

The philosophy from TEKNIKER has been to buy commercial equipment when available and to develop and construct new testing benches, when they are not easily available. Thus, TEKNIKER is equipped with the **most advanced commercial equipment** covering a huge range of testing standards such as:


When possible, round robin tests have been carried out (pin on disc tests, tribocorrosion tests) with different organizations having similar commercial machines.

### **3. New testing benches**

The differential from TEKNIKER is the **capability to develop unique tribological test machines** and new testing configurations to design a wide variety of working conditions (temperature, load, speed) in **different environments** (atmospheric,

**151**

groups.

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

The **new test benches developed by TEKNIKER** have been the following:

• New DEMETRA machine, to measure the **outgassing** of the lubricants,

• **New drag friction** tester to measure drag friction for different applications

• **Tribocorrosimeters** under oscillatory and rotatory conditions, where it is possible to calculate mechanical wear, corrosive (chemical) wear, and the synergy between mechanical wear and chemical wear (UNE 112086, ASTM G119 and

• **Bearing** tests (radial and axial), to measure torque and wear (now in Mecauto-

• **Real bearing friction and wear** test configuration adapted to a Twin Disc and

• **Ball on rod** machine to test point contact fatigue at high pressure and speeds

• **Cylinder on cylinder** to test line contact fatigue at high pressure and speeds

• **Thermal fatigue** test bench, to simulate cycles of high temperature (up to 900°C) and low temperature (the T°C depends on cooling unit selected). One

• **Gravelometer** to test the stone-chip (abrasives, screws) resistance to impact of coatings (paints, varnish) (reference ISO 20567-1:2005). Internal protocols have been developed to test impact resistance in polymer injection molds.

• **Clutch dynamometer** test, to measure torque and wear (now in GOIZPER

machine is available in TEKNIKER and another in AUDI.

(e.g., paints in the ships, friction losses in heat exchangers).

sorption of gases, assisted by mass spectra.

(ASTM E 595, ECSS-Q-ST-70-02C).

internal protocols).

Wisco Company).

Falex machines.

(reference STP 771).

Company).

(12000prm, reference STP 771).

• New atmospheric, vacuum, and ultrahigh **vacuum tribometer** with capacity to test friction and wear at different temperatures and also analyze the tribode-

polymeric materials, and coatings that need to work under vacuum conditions

inert, vacuum, ultrahigh vacuum, corrosive, etc.) in order to cover different tribological problems to analyze the **tribomechanism taking** place on the **rubbed surfaces** (adhesion, die soldering, galling, abrasion, pitting, micropitting, fretting, tribocorrosion, tribodesorption, tribolayer formation, impact, erosion, tactile friction, corrosion, fatigue corrosion, fretting-corrosion, thermal fatigue, fading, etc.). The objective of the measurements carried out with the tribological testing machines is to measure differences in the material behavior. For that, a reference is always used that corresponds to a material with a well-known behavior. The standard deviation of the measurement is established with the reference material. The value of the standard deviation depends on (a) the working conditions (pressure, velocity, temperature, etc.) and (b) the properties (roughness, texturing, composition, etc.). The difference between two materials is significative, if it is higher than three times the standard deviation of the measurements. In some cases, also standard protocols have been developed (e.g., tribocorrosion tests) in collaboration with ISO/CEN

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

inert, vacuum, ultrahigh vacuum, corrosive, etc.) in order to cover different tribological problems to analyze the **tribomechanism taking** place on the **rubbed surfaces** (adhesion, die soldering, galling, abrasion, pitting, micropitting, fretting, tribocorrosion, tribodesorption, tribolayer formation, impact, erosion, tactile friction, corrosion, fatigue corrosion, fretting-corrosion, thermal fatigue, fading, etc.).

The objective of the measurements carried out with the tribological testing machines is to measure differences in the material behavior. For that, a reference is always used that corresponds to a material with a well-known behavior. The standard deviation of the measurement is established with the reference material. The value of the standard deviation depends on (a) the working conditions (pressure, velocity, temperature, etc.) and (b) the properties (roughness, texturing, composition, etc.). The difference between two materials is significative, if it is higher than three times the standard deviation of the measurements. In some cases, also standard protocols have been developed (e.g., tribocorrosion tests) in collaboration with ISO/CEN groups.

The **new test benches developed by TEKNIKER** have been the following:


*Friction, Lubrication and Wear*

D3884 (textiles))

• Ducom **Erosion Tester** (ASTM G-76)

ASTM E303, BS EN 13748-1)

53778, ASTM D 2486, ASTM D 4213)

G96, ASTM G102, ASTM G106)

shore, Norsok), D4585)

**3. New testing benches**

• TABER **abrasion machine** (many standards, e.g., ASTM 4060 (paints), ASTM

• **Pendulum slip** safety testing (UNE-ENV 12663, CEN/TS 16165, BS7976-2,

• GMG **tribometer test for flooring** security (DIN 51131, CEN/TS 16165)

• Microtest **tribometer** transformed by TEKNIKER in a tribocorrosion device

• NEURTEK **Washability** Test, humid rubbing test (UNE-EN ISO 11998, DIN

• CORMET **stress corrosion cracking** in liquid media with electrochemical control until 300°C and autoclave to test stress corrosion at high temperature (800°C) and gaseous media (SO2, NO2, CO2, O2) (ASTM Practice G 129, ASTM

• Metrohm Autolab **potentiostats,** Electrochemical corrosion (ISO 16773-1-4),

(ISO 12944-6), others (ASTM G1, ASTM G3, ASTM G5, ASTM G61, ASTM

• **Climatic chambers** (UV, temperature, humidity, condensation), (e.g., ISO 6270, ASTM D4329, ASTM D4587, ASTM D4799, ASTM D5208, ASTM G151, ASTM G154, DIN EN 12224, DIN EN 1297, DIN EN 13523-10, DIN EN ISO 4892-1, EN 927-6, ISO 11997-2, ISO 16474-3, ISO 4892-3, ISO 20340 (Off

• **INSTRON mechanical tests** at different temperatures at 1–50 kN with speed range 0.005–500 mm/min (many, e.g., tear test (ISO 13937-2:2000))

• Complete laboratory for **paint characterization** to measure impact (e.g., ISO 6272), falling sand abrasive test (e.g., ASTM D 968, ASTM D333; ASTM D1395; ASTM D 2205), crosscut test (e.g., ASTM 3359), bend test (e.g., ISO 6860), Persoz and Kónig hardness (e.g., ISO 1522), pencil scratch test (e.g., ISO 1518-4), cupping test (e.g., EN ISO 1520), pull off test (ISO 4624; ASTM

When possible, round robin tests have been carried out (pin on disc tests, tribocorrosion tests) with different organizations having similar commercial machines.

The differential from TEKNIKER is the **capability to develop unique tribological test machines** and new testing configurations to design a wide variety of working conditions (temperature, load, speed) in **different environments** (atmospheric,

liquid corrosion (ISO 2812-1, ISO 2812-2), corrosion classification

Test Method E8). NACE Standards (TM0198, TM0177)

• **Compatibility of seals** with lubricants (ASTM D471)

D4541), brightness loss (Crock meter)

• Corrosion test salt spray (ISO 9227, ASTM B117)

**150**


### **4. Description of the main new test benches**

### **4.1 CATRI (CA3UHV) machine**

CATRI (CA3UHV) machine has been developed by TEKNIKER to determine the friction and wear properties in atmospheric, vacuum, and ultrahigh vacuum conditions. It is also possible to measure the gas tribodesorption detected by mass spectra, during friction and wear tests. Both the force sensor and sample holder of the experimental system have been patented, PCT/ES2009/070635 and PCT/ES2010/07273, respectively [1–4]. In this machine, the patents from CSIC ES200700480 and ES2320513B1 have also been validated. This machine allows complex tribological characterization of materials and coatings in a wide range of gas pressures from atmospheric to ultrahigh vacuum and loads (0.1–20 N). This system can be used to study tribological behavior of the coatings under gradually varying gas pressure and composition, simulating the environments on the various stages of the service life of the real aerospace systems. The machine can work under ultrahigh vacuum (5 × 10<sup>−</sup>10 mbar) and inert gas in controlled atmosphere (from 103 to 5 × 10<sup>−</sup><sup>9</sup> hPa). T°C can reach up to 350°C. It can be possible to quantify the gas tribodesorption from materials and coatings (**Figure 1**).

**153**

**Figure 3.**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

DEMETRA machine is developed for the analysis of the outgassing from lubricants and materials (e.g., coatings, textiles, and plastics) in vacuum conditions. The bench test has been built using the ASTM E595-07 and ECSS-Q-ST-70-02C Reference Protocols. In the test, the volatile components of the materials and lubricants are determined at 125°C in vacuum conditions. The flexibility of the machine allows to modify working conditions. According to the standard, the Recovered mass loss (RML) should be <1% and the Collected volatile condensable material

Drag friction test is for the determination of the drag friction torque of antifouling paints or surface treatments (e.g., texturing). The test samples are hollowed cylinders of 200 × 200 m that can be either located in ships or in the port to be covered with fouling after a specific time period. The torque before and after fouling and with different surface treatments can be compared at different rotating speeds, simulating either laminar or turbulent flow. Two test configurations are available with gaps of 5 and 10 mm. The machine has been developed by TEKNIKER in the frame of EU Project Foul X PEL (https://cordis.europa.eu/project/rcn/101484/reporting/en) (**Figure 3**) [5, 6].

*Details of (a) vacuum chamber, (b) evaporation unit with four testing stations, and (c) DEMETRA machine* 

Tribocorrosion testers have been developed combining a tribometer and a poten-

tiostat. The test equipment allows monitoring and control both mechanical and electrochemical parameters. A tribometer creates relative motion, either unidirectional (rotatory) or bidirectional (reciprocating), rubbing two surfaces against each

*(a) Drag friction tester, TEKNIKER©. (b) The image shows the testing cylinder location in a ship.*

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

(CVCM) should be <0.1% (**Figure 2**) [3].

**4.2 DEMETRA machine**

**4.3 Drag friction test**

*developed by TEKNIKER.*

**Figure 2.**

**4.4 Tribocorrosion testers**

**Figure 1.** *(a) CATRI machine, (b) detail of the sample holder, TEKNIKER©.*

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

### **4.2 DEMETRA machine**

*Friction, Lubrication and Wear*

temperatures.

and SRV machines.

**4.1 CATRI (CA3UHV) machine**

atmosphere (from 103

solar mirrors (internal protocols).

**4. Description of the main new test benches**

to 5 × 10<sup>−</sup><sup>9</sup>

*(a) CATRI machine, (b) detail of the sample holder, TEKNIKER©.*

• **Disc brake** dynamometer test bench, to measure the friction, wear, and thermal fatigue of disc brakes (now in Edertek-Fagor Ederlan company).

piston skirt/cylinder liner, impact of valve seat/valve head, etc.

• **New seals** test bench under reciprocating and oscillatory movement with capacity to test with different lubrication systems and different

• **Prosthesis simulators** involving real components for evaluating tribological properties of hip prosthesis coatings and synovial fluids, adapted to FALEX

• **Car wash type test,** cleaning and abrasive testing of glass (ISO 20566) and

CATRI (CA3UHV) machine has been developed by TEKNIKER to determine the friction and wear properties in atmospheric, vacuum, and ultrahigh vacuum conditions. It is also possible to measure the gas tribodesorption detected by mass spectra, during friction and wear tests. Both the force sensor and sample holder of the experimental system have been patented, PCT/ES2009/070635 and PCT/ES2010/07273, respectively [1–4]. In this machine, the patents from CSIC ES200700480 and ES2320513B1 have also been validated. This machine allows complex tribological characterization of materials and coatings in a wide range of gas pressures from atmospheric to ultrahigh vacuum and loads (0.1–20 N). This system can be used to study tribological behavior of the coatings under gradually varying gas pressure and composition, simulating the environments on the various stages of the service life of the real aerospace systems. The machine can work under ultrahigh vacuum (5 × 10<sup>−</sup>10 mbar) and inert gas in controlled

sible to quantify the gas tribodesorption from materials and coatings (**Figure 1**).

hPa). T°C can reach up to 350°C. It can be pos-

• Testing configurations of **engine component** wear and friction test have been adapted to the SRV, FALEX, and CETR machines (e.g., ASTM G181-11, ASTM G206-17). Several new protocols have been developed to simulate valve stem/ guide, gudgeon pin/piston, piston ring/cylinder liner, piston ring/piston,

**152**

**Figure 1.**

DEMETRA machine is developed for the analysis of the outgassing from lubricants and materials (e.g., coatings, textiles, and plastics) in vacuum conditions. The bench test has been built using the ASTM E595-07 and ECSS-Q-ST-70-02C Reference Protocols. In the test, the volatile components of the materials and lubricants are determined at 125°C in vacuum conditions. The flexibility of the machine allows to modify working conditions. According to the standard, the Recovered mass loss (RML) should be <1% and the Collected volatile condensable material (CVCM) should be <0.1% (**Figure 2**) [3].

**Figure 2.**

*Details of (a) vacuum chamber, (b) evaporation unit with four testing stations, and (c) DEMETRA machine developed by TEKNIKER.*

### **4.3 Drag friction test**

Drag friction test is for the determination of the drag friction torque of antifouling paints or surface treatments (e.g., texturing). The test samples are hollowed cylinders of 200 × 200 m that can be either located in ships or in the port to be covered with fouling after a specific time period. The torque before and after fouling and with different surface treatments can be compared at different rotating speeds, simulating either laminar or turbulent flow. Two test configurations are available with gaps of 5 and 10 mm. The machine has been developed by TEKNIKER in the frame of EU Project Foul X PEL (https://cordis.europa.eu/project/rcn/101484/reporting/en) (**Figure 3**) [5, 6].

**Figure 3.** *(a) Drag friction tester, TEKNIKER©. (b) The image shows the testing cylinder location in a ship.*

### **4.4 Tribocorrosion testers**

Tribocorrosion testers have been developed combining a tribometer and a potentiostat. The test equipment allows monitoring and control both mechanical and electrochemical parameters. A tribometer creates relative motion, either unidirectional (rotatory) or bidirectional (reciprocating), rubbing two surfaces against each

### *Friction, Lubrication and Wear*

other. The electrochemical cells are used to record and control the electrochemical parameters. These cells are usually composed of three electrodes: a reference electrode, a counter-electrode, and the working electrode. The reference electrode has a stable, well-defined potential, and it is used to register the potential of the working electrode, i.e., the test sample. Typical reference electrodes are saturated calomel electrodes (SCE) and silver/silver chloride electrodes (Ag/AgCl). The counter-electrode is used to measure or control the current and is usually made of inert materials such as platinum, gold, or graphite. The electrodes are connected to a potentiostat to register the potential between the reference electrode and the working electrode or the current between the counter-electrode and the working electrode. A typical tribocorrosion test setup is schematically shown in **Figure 4** [7–16].

**Figure 4.**

*Experimental setup of a tribocorrosion device for a unidirectional tribometer under ball on disc configuration, TEKNIKER©.*

### **4.5 Test bench for plain bearings**

A test bench is built with the objective to carry out friction test and wear test in plain bearings. Alternative movement has a stroke of 120–125 mm, a speed of 1–40 m/min, and a maximum load of 3000 kgf (**Figure 5**) [17, 18].

**Figure 5.** *Plain bearing testing machine, designed and constructed by TEKNIKER for Mecauto-Wisco company.*

### **4.6 Ball on rod machine**

Ball on rod machine is built with the objective to study the point rolling contact fatigue of the bearing materials and coatings, to apply to ball rolling bearings. It follows

**155**

**Figure 7.**

**Figure 6.**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

Cylinder on cylinder machine, built to study the pitting phenomena in roller bearings, simulates the line contact rolling fatigue behavior of the materials. The machine is based on ASTM STP 771 protocol, with the advantage of reaching a maximum speed of 12,000 rpm with air/oil lubrication. The roller's size is 12x12mm. The duration of the test until reaching the micropitting or pitting phenomena is recorded for different types of materials and coatings of the rollers. The test stops, when the level of vibration increases, due to generation of pitting in the contact. The machine was developed by TEKNIKER in collaboration with SKF, in the frame of EU Project REFINE (**Figure 7**) (https://cordis.europa.eu/project/rcn/36428/factsheet/en).

the protocol from Douglas Glover, "A Ball-Rod Rolling Contact Fatigue Tester" (ASTM STP 771, J. J. C. Hoo, D., American Society for Testing and Materials, 1982, pp. 107–124). It has a variable speed, reaching up to 12,000 rpm instead of 3000 rpm of the documented protocol. The typical pressure applied is 5.5 MPa. The lubrication is an air/oil system with controlled flow, typical lubrication regime for high-speed rolling bearings. Alternatively, other lubrication systems can be selected. The balls can be made from steel and ceramic and with or without coatings with a diameter of 12.7 mm. The roller has a diameter of 10 mm and length of 125 mm. The ball on rod machine has a double testing device for parallel testing. The time to reach the micropitting or pitting is recorded and monitored by an increase of the vibrations. The machine was developed by TEKNIKER in collaboration with SNR, in the frame of EU Project Eurobearing (https://cordis.europa.eu/project/rcn/6657/factsheet/es) (**Figure 6**) [19].

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

**4.7 Cylinder on cylinder machine**

*Ball on rod machine, TEKNIKER©.*

*(a) Cylinder on cylinder machine, TEKNIKER©, (b) pitting in a roller.*

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

the protocol from Douglas Glover, "A Ball-Rod Rolling Contact Fatigue Tester" (ASTM STP 771, J. J. C. Hoo, D., American Society for Testing and Materials, 1982, pp. 107–124). It has a variable speed, reaching up to 12,000 rpm instead of 3000 rpm of the documented protocol. The typical pressure applied is 5.5 MPa. The lubrication is an air/oil system with controlled flow, typical lubrication regime for high-speed rolling bearings. Alternatively, other lubrication systems can be selected. The balls can be made from steel and ceramic and with or without coatings with a diameter of 12.7 mm. The roller has a diameter of 10 mm and length of 125 mm. The ball on rod machine has a double testing device for parallel testing. The time to reach the micropitting or pitting is recorded and monitored by an increase of the vibrations. The machine was developed by TEKNIKER in collaboration with SNR, in the frame of EU Project Eurobearing (https://cordis.europa.eu/project/rcn/6657/factsheet/es) (**Figure 6**) [19].

**Figure 6.** *Ball on rod machine, TEKNIKER©.*

*Friction, Lubrication and Wear*

**4.5 Test bench for plain bearings**

other. The electrochemical cells are used to record and control the electrochemical parameters. These cells are usually composed of three electrodes: a reference electrode, a counter-electrode, and the working electrode. The reference electrode has a stable, well-defined potential, and it is used to register the potential of the working electrode, i.e., the test sample. Typical reference electrodes are saturated calomel electrodes (SCE) and silver/silver chloride electrodes (Ag/AgCl). The counter-electrode is used to measure or control the current and is usually made of inert materials such as platinum, gold, or graphite. The electrodes are connected to a potentiostat to register the potential between the reference electrode and the working electrode or the current between the counter-electrode and the working electrode. A typical

A test bench is built with the objective to carry out friction test and wear test in plain bearings. Alternative movement has a stroke of 120–125 mm, a speed of

*Experimental setup of a tribocorrosion device for a unidirectional tribometer under ball on disc configuration,* 

Ball on rod machine is built with the objective to study the point rolling contact fatigue of the bearing materials and coatings, to apply to ball rolling bearings. It follows

*Plain bearing testing machine, designed and constructed by TEKNIKER for Mecauto-Wisco company.*

1–40 m/min, and a maximum load of 3000 kgf (**Figure 5**) [17, 18].

tribocorrosion test setup is schematically shown in **Figure 4** [7–16].

**154**

**Figure 5.**

**Figure 4.**

*TEKNIKER©.*

**4.6 Ball on rod machine**

### **4.7 Cylinder on cylinder machine**

Cylinder on cylinder machine, built to study the pitting phenomena in roller bearings, simulates the line contact rolling fatigue behavior of the materials. The machine is based on ASTM STP 771 protocol, with the advantage of reaching a maximum speed of 12,000 rpm with air/oil lubrication. The roller's size is 12x12mm. The duration of the test until reaching the micropitting or pitting phenomena is recorded for different types of materials and coatings of the rollers. The test stops, when the level of vibration increases, due to generation of pitting in the contact. The machine was developed by TEKNIKER in collaboration with SKF, in the frame of EU Project REFINE (**Figure 7**) (https://cordis.europa.eu/project/rcn/36428/factsheet/en).

**Figure 7.** *(a) Cylinder on cylinder machine, TEKNIKER©, (b) pitting in a roller.*

### **4.8 The thermal fatigue**

The thermal fatigue test bench has been built to simulate thermal cycles of high temperature generated by induction heating and low temperature cooled with spray. There is one machine in TEKNIKER and one in AUDI. The machine has been developed to simulate the heating and cooling cycles of the high pressure die casting dies. The time to thermal fatigue crack failure mainly depends on (a) the maximum temperature, (b) the temperature gradient, (c) the geometry, and (d) the designed cooling channels inside the mold (testing block). The machine can simulate a time to thermal fatigue failure similar to the real applications (**Figure 8**) [20].

**Figure 8.** *(a) Cooling process, (b) heating process of the thermal fatigue machine TEKNIKER©.*

### **4.9 Brake disc testing machine**

Brake disc testing machine is built with the objective of carrying out friction, wear, and thermal fatigue tests of disc brakes and brake drums. The maximum velocity is 2500 rpm and the maximum load is 105 kg/m<sup>2</sup> . During the test, the torque and the temperature and wear are recorded. Different protocols from automotive suppliers can be applied (e.g., AUDI, Volkswagen) (**Figure 9**) [21].

**Figure 9.** *Disc brake testing machine, designed and constructed by TEKNIKER for Fagor Ederlan company.*

### **4.10 Clutch dynamometer test**

Clutch dynamometer test has been built with the objective to measure the friction and wear of the clutches at fixed or variable conditions of load and speed.

**157**

**Figure 11.**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

Measurement of force, the friction loss between the cylinder and braking films, and temperatures at different points, forces, torque, and speeds are recorded. The specific power, specific energy, the dynamic and static torques, the sliding time, and initial speed can be monitored during breaking or evaluated during the test

The TESSA machine has been developed by TEKNIKER to measure the friction, wear, and leakage of the dynamic seals [23–28]. It can reach a maximum speed of 6 m/s. The machine has been adapted to work under variable temperature integrating a climatic chamber. The test chamber is modular, and it has the capability to measure the differential pressure between the two sides of the seals for pistons and rollers and evaluate the leakage. Oils sensors, developed by TEKNIKER (www. tekniker.es/en/ and ATTEN2 (https://atten2.com/en/), can be used to monitor the

*(a) Clutch dynamometer test bench. (b) Control unit of the dynamometer, constructed by TEKNIKER for* 

Glass and mirror wash test has been built to evaluate the scratch abrasion resistance of coatings used in glass of the cars and solar mirrors. In automotive sector, the glass car wash resistance is assessed. A machine-based washing is simulated in the laboratory environment using a rotating brush and synthetic dirt. The test conditions have been designed to be as close as possible to the real conditions in a car wash and solar mirrors, in order to evaluate the cleanability, the abrasion resistance, and their durability. Protocols for solar mirror evaluation are under development by TEKNIKER

*(a) New seal test bench constructed by TEKNIKER with two units with oscillatory and reciprocal movements* 

*and climatic temperature control (low and high temperatures). (b) Example of test conditions.*

in the frame of EU Project In Power (http://in-power-project.eu/) (**Figure 12**).

generation of wear particles in lubricated seals (**Figure 11**).

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

(**Figure 10**) [22].

**Figure 10.**

*GOIZPER company.*

**4.11 The TESSA machine**

**4.12 Glass and mirror wash test**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

Measurement of force, the friction loss between the cylinder and braking films, and temperatures at different points, forces, torque, and speeds are recorded. The specific power, specific energy, the dynamic and static torques, the sliding time, and initial speed can be monitored during breaking or evaluated during the test (**Figure 10**) [22].

### **Figure 10.**

*Friction, Lubrication and Wear*

**4.8 The thermal fatigue**

**4.9 Brake disc testing machine**

**Figure 8.**

**4.10 Clutch dynamometer test**

velocity is 2500 rpm and the maximum load is 105 kg/m<sup>2</sup>

*(a) Cooling process, (b) heating process of the thermal fatigue machine TEKNIKER©.*

The thermal fatigue test bench has been built to simulate thermal cycles of high

Brake disc testing machine is built with the objective of carrying out friction, wear, and thermal fatigue tests of disc brakes and brake drums. The maximum

torque and the temperature and wear are recorded. Different protocols from auto-

Clutch dynamometer test has been built with the objective to measure the friction and wear of the clutches at fixed or variable conditions of load and speed.

*Disc brake testing machine, designed and constructed by TEKNIKER for Fagor Ederlan company.*

motive suppliers can be applied (e.g., AUDI, Volkswagen) (**Figure 9**) [21].

. During the test, the

temperature generated by induction heating and low temperature cooled with spray. There is one machine in TEKNIKER and one in AUDI. The machine has been developed to simulate the heating and cooling cycles of the high pressure die casting dies. The time to thermal fatigue crack failure mainly depends on (a) the maximum temperature, (b) the temperature gradient, (c) the geometry, and (d) the designed cooling channels inside the mold (testing block). The machine can simulate a time

to thermal fatigue failure similar to the real applications (**Figure 8**) [20].

**156**

**Figure 9.**

*(a) Clutch dynamometer test bench. (b) Control unit of the dynamometer, constructed by TEKNIKER for GOIZPER company.*

### **4.11 The TESSA machine**

The TESSA machine has been developed by TEKNIKER to measure the friction, wear, and leakage of the dynamic seals [23–28]. It can reach a maximum speed of 6 m/s. The machine has been adapted to work under variable temperature integrating a climatic chamber. The test chamber is modular, and it has the capability to measure the differential pressure between the two sides of the seals for pistons and rollers and evaluate the leakage. Oils sensors, developed by TEKNIKER (www. tekniker.es/en/ and ATTEN2 (https://atten2.com/en/), can be used to monitor the generation of wear particles in lubricated seals (**Figure 11**).

**Figure 11.**

*(a) New seal test bench constructed by TEKNIKER with two units with oscillatory and reciprocal movements and climatic temperature control (low and high temperatures). (b) Example of test conditions.*

### **4.12 Glass and mirror wash test**

Glass and mirror wash test has been built to evaluate the scratch abrasion resistance of coatings used in glass of the cars and solar mirrors. In automotive sector, the glass car wash resistance is assessed. A machine-based washing is simulated in the laboratory environment using a rotating brush and synthetic dirt. The test conditions have been designed to be as close as possible to the real conditions in a car wash and solar mirrors, in order to evaluate the cleanability, the abrasion resistance, and their durability. Protocols for solar mirror evaluation are under development by TEKNIKER in the frame of EU Project In Power (http://in-power-project.eu/) (**Figure 12**).

**Figure 12.** *Glass and solar mirror testing device TEKNIKER©.*

### **5. Case studies**

Different case studies have been selected to cover examples of different tribological characterization tools and equipment used for material selection (composition, topography, surface treatments, lubricants), making emphasis in the failure mechanism and friction simulation of a wide variety of materials, tribological systems, and environments.

### **5.1 Tribology for aggressive environments**

### *5.1.1 Vacuum and ultrahigh vacuum tribology*

The **CATRI tribometer** (see **Figure 1**) has been used to screen the tribological properties under vacuum and ultrahigh vacuum of the steel/coating and titanium materials lubricated with different fluids (oils, greases, or ionic liquids). For example, it has been observed that it is possible to find non-halogen ionic liquids to lubricate steel under vacuum and ultrahigh vacuum conditions (e.g., phosphonium phosphate) and to lubricate titanium; up to now, better results have been obtained with halogen-containing ionic liquids or lubricants (e.g., [Bu3MeP][Tf2N]). The desorption of CF3 detected in the mass spectra occurred just in the moment when the friction was reduced (see **Figure 13a**). During the test, a TiFx tribolayer was generated. Titanium and inorganic F and S(II) were detected by XPS. The reaction mechanism that explained the TiFx layer generation was elucidated (see **Figure 13c**) thanks to the fragments of the mass spectra (see **Figure 13b**) detected during the tribodesorption process. The machine and protocols have been used in the National Project CATRI [1], the EU Project MINILUBES [2], the Austrian X-Tribology COMET Initiative [3], the Eurostars Project VACUUM DLC [4], and industrial projects.

### **Figure 13.**

*(a) Friction coefficient during ultrahigh vacuum tribotest (b) mass spectra, highlighting the hydrogen and CF3 fragments from the F-containing lubricant. (c) Proposed tribomechanism for the TiFx generation.*

**159**

**Figure 15.**

(**Figure 15**).

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

The DEMETRA machine (see **Figure 2**) was built to measure the **outgassing under vacuum** to screen and select the materials and lubricants that can work under these conditions. The volatility data of the outgassing measurements of the ionic liquid [Bu3MeP][Tf2N] has been compared to the reference lubricant, a perfluoropolyether (PFPE). It can be stated that the ionic liquid exhibits acceptable outgassing data according to the requirements of the standard ASTM E595 (RML <1.0% and CVCM <0.1%) [3]. The machine has been used in EU Projects VACUUM DLC and Austrian X-Tribology COMET Initiative. It has also been used to study dependence of outgassing of thermal fluids in function of the viscosity for heat exchangers (see Section 11.2) in EU Project SUSPIRE (http://suspire-h2020.eu/)

The development of the **drag friction test** (see **Figure 3**) has been carried out in the frame of EU Project FOUL X PEL [5, 6]. In this study, the torque of different antifouling paints before and after immersion in a ship or in the Motrico Port has been compared. The tests have been carried out with artificial sea water fluid (ASTM D1141) in a container under rotation at different speed, generating laminar or turbulent regime, using different gaps of 5 and 10 mm. The effect of biofouling, roughness, and fluid properties can be measured. In the example, two fluids FX1 and FX2 were tested and being selected FX2 due to their lower drag friction in all the range of speeds tested. The machine has also been used in the EU Project SUSPIRE to test thermal fluids with different viscosities to select those with lower drag friction loss and higher energy efficiency (see Section 11.2)

*Comparative drag friction measurement of two antifouling coatings, before and after 1-year sea exposure in a ship.*

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

*5.1.3 Drag friction tribology in marine environments*

*Outgassing data of the PFPE oil and the ionic liquid (ASTM E595).*

*5.1.2 The DEMETRA machine*

(**Figure 14**).

**Figure 14.**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

### *5.1.2 The DEMETRA machine*

*Friction, Lubrication and Wear*

**5. Case studies**

**Figure 12.**

systems, and environments.

**5.1 Tribology for aggressive environments**

*Glass and solar mirror testing device TEKNIKER©.*

*5.1.1 Vacuum and ultrahigh vacuum tribology*

Different case studies have been selected to cover examples of different tribological characterization tools and equipment used for material selection (composition, topography, surface treatments, lubricants), making emphasis in the failure mechanism and friction simulation of a wide variety of materials, tribological

The **CATRI tribometer** (see **Figure 1**) has been used to screen the tribological properties under vacuum and ultrahigh vacuum of the steel/coating and titanium materials lubricated with different fluids (oils, greases, or ionic liquids). For example, it has been observed that it is possible to find non-halogen ionic liquids to lubricate steel under vacuum and ultrahigh vacuum conditions (e.g., phosphonium phosphate) and to lubricate titanium; up to now, better results have been obtained with halogen-containing ionic liquids or lubricants (e.g., [Bu3MeP][Tf2N]). The desorption of CF3 detected in the mass spectra occurred just in the moment when the friction was reduced (see **Figure 13a**). During the test, a TiFx tribolayer was generated. Titanium and inorganic F and S(II) were detected by XPS. The reaction mechanism that explained the TiFx layer generation was elucidated (see **Figure 13c**) thanks to the fragments of the mass spectra (see **Figure 13b**) detected during the tribodesorption process. The machine and protocols have been used in the National Project CATRI [1], the EU Project MINILUBES [2], the Austrian X-Tribology COMET Initiative [3], the Eurostars Project VACUUM DLC [4], and industrial projects.

*(a) Friction coefficient during ultrahigh vacuum tribotest (b) mass spectra, highlighting the hydrogen and CF3*

*fragments from the F-containing lubricant. (c) Proposed tribomechanism for the TiFx generation.*

**158**

**Figure 13.**

The DEMETRA machine (see **Figure 2**) was built to measure the **outgassing under vacuum** to screen and select the materials and lubricants that can work under these conditions. The volatility data of the outgassing measurements of the ionic liquid [Bu3MeP][Tf2N] has been compared to the reference lubricant, a perfluoropolyether (PFPE). It can be stated that the ionic liquid exhibits acceptable outgassing data according to the requirements of the standard ASTM E595 (RML <1.0% and CVCM <0.1%) [3]. The machine has been used in EU Projects VACUUM DLC and Austrian X-Tribology COMET Initiative. It has also been used to study dependence of outgassing of thermal fluids in function of the viscosity for heat exchangers (see Section 11.2) in EU Project SUSPIRE (http://suspire-h2020.eu/) (**Figure 14**).


**Figure 14.**

*Outgassing data of the PFPE oil and the ionic liquid (ASTM E595).*

### *5.1.3 Drag friction tribology in marine environments*

The development of the **drag friction test** (see **Figure 3**) has been carried out in the frame of EU Project FOUL X PEL [5, 6]. In this study, the torque of different antifouling paints before and after immersion in a ship or in the Motrico Port has been compared. The tests have been carried out with artificial sea water fluid (ASTM D1141) in a container under rotation at different speed, generating laminar or turbulent regime, using different gaps of 5 and 10 mm. The effect of biofouling, roughness, and fluid properties can be measured. In the example, two fluids FX1 and FX2 were tested and being selected FX2 due to their lower drag friction in all the range of speeds tested. The machine has also been used in the EU Project SUSPIRE to test thermal fluids with different viscosities to select those with lower drag friction loss and higher energy efficiency (see Section 11.2) (**Figure 15**).

**Figure 15.**

*Comparative drag friction measurement of two antifouling coatings, before and after 1-year sea exposure in a ship.*

### *5.1.4 Tribocorrosion*

The coupling of standard tribometers with a potentiostat has been done to measure **wear-corrosion** behaviour, that means to study the mechanical, the chemical wear and the synergy between both phenomena. In the frame of RAMPE Project [11], the tribocorrosion properties of Inconel + Cr electrodeposited coating is compared with CrN+TiN coating deposited by Physical Vapour Deposition (PVD) developed by TEKNIKER. It is observed that the impedance (corrosion resistance) after the wear test, is considerably reduced for Inconel + Cr Coating. In case of CrN+TiN PVD coating, the impedance curve resulted unaltered after wear test. These results correlate well with the wear scars measured after the test, for both coatings (see **Figure 16**). The technique has been used also in EU Projects FUNCOAT [7, 29–31], FRONTIERS [10], NADIA [32], in Regional project TRICONDEX [8], FRONTIERS [12], and National project NANOTRIBOCOR [9].

**Figure 16.**

*Impedance measurements before and after wear test for (a) Inconel + Cr coating and (b) Inconel + PVD TiN + CrN coating. Wear scars: (c) Inconel + Cr and (d) Inconel + TiN/CrN coating.*

### *5.1.5 Tribocorrosion in marine and offshore environments*

High-strength low-alloy (HSLA) steels employed in offshore applications suffer high degradation due to their high corrosivity in seawater and the wear generated during mooring chain movement. The results, obtained in the frame of the FONDEO Adhoc project financed by the Spanish Minister of Science, showed an acceleration of corrosion during wear experiments, as consequence of the synergism generated between wear and corrosion. In **Figure 17(***i***)**, it can be seen, how the sliding has modified the electrochemical behavior of both steels. The effect of several parameters such as seawater temperature or salinity have also been studied to understand their

### **Figure 17.**

*(i) Potentiodynamic polarization curves obtained for two HSLA steel grades (R4 and R5) under corrosion (without sliding) and under tribocorrosion (with sliding) in synthetic seawater. (j) Topography of the wear tracks obtained after tribocorrosion tests on: (a) the TSA and (b) PEO-treated TSA.*

**161**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

influence in the steel degradation [13, 14]. In order to protect steels in mooring lines of floating structures, it has been developed some surface treatments based on thermally sprayed aluminum (TSA) coating with and without post-treatment by plasma electrolytic oxidation (PEO). In **Figure 17(***j***)**, it can be highlighted the reduction of wear scar after tribocorrosion tests, can be highlighted and produced when the TSA coating on the steel is additionally treated by plasma electrooxidation (**Figure 17(***jb***)**) [15, 16].

Two testing benches have been constructed (see **Figure 4**) for Mecauto company to study the torque and wear in axial and radial bearings. Also, a standard tribotest has been adapted to study the limits of pressure and velocity of the tribological pair. In the frame of BELEADFREE Project, a test has been designed to evaluate the tribological properties of real bearings. In the frame of EREBIO EU Project, the reduction of friction and contact temperature has been proven when using a biodegradable low-viscosity and environmentally friendly engine oil for the lubrication of bearings using a basic thrust washer configuration [17]. In the project ECOBEARINGS [18] and BELEADFREE, the lead content of the bearings have been

As described before, the ball on rod (**Figure 6**) and cylinder on cylinder machines (**Figure 7**) have been constructed by TEKNIKER to study point and line contact rolling fatigue to understand the pitting failure behavior of rolling bearing materials, under high contact loads and high speeds. In the frame of EUROBEARING project, different PVD coatings were studied, measuring the load-carrying capacity, the adherence, the abrasion resistance, and the hardness, as shown in the next table. Their fatigue resistance was also tested using the ball on rod machine. The long fatigue lifetime (1000 million cycles duration) of the TiN + C coating and their good behavior against abrasion and adhesion make this coating a promising alternative to be applied in high-speed rolling bearings [19] (**Table 1**). In this subject, (a) the relationship between vibration generation and oil particle generation (EU Projects TESS) [33], (b) the fatigue behavior of roller bearings (REFINE), and (c) the behavior of different PVD coatings and lubricants for rolling bearings (National Project HIEFBE) have been studied, and (d) a test

*Evolution of temperature when using biodegradable and mineral lubricants to lubricate journal bearings.*

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

**5.2. Tribology of mechanical components**

*5.2.1 Tribology of journal bearings*

reduced or eliminated (**Figure 18**).

*5.2.2 Tribology of rolling bearings*

**Figure 18.**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

influence in the steel degradation [13, 14]. In order to protect steels in mooring lines of floating structures, it has been developed some surface treatments based on thermally sprayed aluminum (TSA) coating with and without post-treatment by plasma electrolytic oxidation (PEO). In **Figure 17(***j***)**, it can be highlighted the reduction of wear scar after tribocorrosion tests, can be highlighted and produced when the TSA coating on the steel is additionally treated by plasma electrooxidation (**Figure 17(***jb***)**) [15, 16].

### **5.2. Tribology of mechanical components**

### *5.2.1 Tribology of journal bearings*

*Friction, Lubrication and Wear*

The coupling of standard tribometers with a potentiostat has been done to measure **wear-corrosion** behaviour, that means to study the mechanical, the chemical wear and the synergy between both phenomena. In the frame of RAMPE Project [11], the tribocorrosion properties of Inconel + Cr electrodeposited coating is compared with CrN+TiN coating deposited by Physical Vapour Deposition (PVD) developed by TEKNIKER. It is observed that the impedance (corrosion resistance) after the wear test, is considerably reduced for Inconel + Cr Coating. In case of CrN+TiN PVD coating, the impedance curve resulted unaltered after wear test. These results correlate well with the wear scars measured after the test, for both coatings (see **Figure 16**). The technique has been used also in EU Projects FUNCOAT [7, 29–31], FRONTIERS [10], NADIA [32], in Regional project TRICONDEX [8], FRONTIERS [12], and National project NANOTRIBOCOR [9].

*5.1.5 Tribocorrosion in marine and offshore environments*

*TiN + CrN coating. Wear scars: (c) Inconel + Cr and (d) Inconel + TiN/CrN coating.*

High-strength low-alloy (HSLA) steels employed in offshore applications suffer high degradation due to their high corrosivity in seawater and the wear generated during mooring chain movement. The results, obtained in the frame of the FONDEO Adhoc project financed by the Spanish Minister of Science, showed an acceleration of corrosion during wear experiments, as consequence of the synergism generated between wear and corrosion. In **Figure 17(***i***)**, it can be seen, how the sliding has modified the electrochemical behavior of both steels. The effect of several parameters such as seawater temperature or salinity have also been studied to understand their

*(i) Potentiodynamic polarization curves obtained for two HSLA steel grades (R4 and R5) under corrosion (without sliding) and under tribocorrosion (with sliding) in synthetic seawater. (j) Topography of the wear* 

*tracks obtained after tribocorrosion tests on: (a) the TSA and (b) PEO-treated TSA.*

*Impedance measurements before and after wear test for (a) Inconel + Cr coating and (b) Inconel + PVD* 

*5.1.4 Tribocorrosion*

**Figure 16.**

**160**

**Figure 17.**

Two testing benches have been constructed (see **Figure 4**) for Mecauto company to study the torque and wear in axial and radial bearings. Also, a standard tribotest has been adapted to study the limits of pressure and velocity of the tribological pair. In the frame of BELEADFREE Project, a test has been designed to evaluate the tribological properties of real bearings. In the frame of EREBIO EU Project, the reduction of friction and contact temperature has been proven when using a biodegradable low-viscosity and environmentally friendly engine oil for the lubrication of bearings using a basic thrust washer configuration [17]. In the project ECOBEARINGS [18] and BELEADFREE, the lead content of the bearings have been reduced or eliminated (**Figure 18**).

**Figure 18.** *Evolution of temperature when using biodegradable and mineral lubricants to lubricate journal bearings.*

### *5.2.2 Tribology of rolling bearings*

As described before, the ball on rod (**Figure 6**) and cylinder on cylinder machines (**Figure 7**) have been constructed by TEKNIKER to study point and line contact rolling fatigue to understand the pitting failure behavior of rolling bearing materials, under high contact loads and high speeds. In the frame of EUROBEARING project, different PVD coatings were studied, measuring the load-carrying capacity, the adherence, the abrasion resistance, and the hardness, as shown in the next table. Their fatigue resistance was also tested using the ball on rod machine. The long fatigue lifetime (1000 million cycles duration) of the TiN + C coating and their good behavior against abrasion and adhesion make this coating a promising alternative to be applied in high-speed rolling bearings [19] (**Table 1**). In this subject, (a) the relationship between vibration generation and oil particle generation (EU Projects TESS) [33], (b) the fatigue behavior of roller bearings (REFINE), and (c) the behavior of different PVD coatings and lubricants for rolling bearings (National Project HIEFBE) have been studied, and (d) a test


configuration to study the tribology of real bearings has been developed, adapted to FALEX tribological test (Project BIOMON).

**Table 1.**

*Qualitative behavior of coatings to increase lifetime of rolling bearings [19].*

### *5.2.3 Tribology of clutches and brakes*

Brakes and clutches require high stable friction coefficient. To understand the tribology phenomena of these systems, testing protocols have been developed for the standard FALEX (high-performance and multispecimen) tribometers to study the friction wear mechanism of brakes and clutches (high temperature abrasion, adhesion, and fading) and to study the relationship of the friction coefficient with the squeal generation. Additionally, a dynamometer test bench has been constructed to test disc brakes (**Figure 9**) and clutches (**Figure 10**). In the frame of the i-SINTER Project, the correlation between the friction measured in pin on disc tests and the torque measured in clutch tests has been studied, observing very similar values, especially at low loads (**Figure 19**). These conditions were selected for screening of the materials with pin on disc tests, before final validation in the clutch test. The tribological knowledge on dry friction has been used in the projects M-eranet JOLIE (brakes) [21], Manunet BRAKE SQUEAL (clutches) [22], and Industrial Project I-SINTER (clutches).

**163**

**Figure 21.**

*block of the mold material after 10,000 thermal cycles.*

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

[34], EREBIO [35–37], VOSOLUB [38], SUNOIL [39], LUBRICOAT [40], BIOGREASE [39], and BIOMON [41] and the industrial projects AEROHUMs

*5.3.1 Tribology of high-pressure die casting (HPDC) and polymer injection molds* 

*a) Upgrading of FZG machine to monitor vibration, transmission error, power losses, noise, temperature, and* 

In the frame of MUSIC Project, a thermal fatigue machine has been constructed to reproduce the main failure of the high-pressure die casting molds. In **Figure 21a**, the thermal cycles can be seen in high-pressure die casting process reproduced in the thermal fatigue machine, and in **Figure 21b**, the thermal fatigue mechanism can be observed, reproduced in a flat specimen with internal cooling circuits, representing the die. The thermal fatigue mechanism can also be reproduced in 3D complex geometries. Setup of testing protocols has been carried out to simulate also other failure mechanisms of HPDC and PIM molds such as mechanical and chemical die soldering, abrasion and erosion resistance, and the corrosion behavior. The knowledge generated in MUSIC project has been applied to the EUROSTAR Project

*(a) Thermal cycles in the thermal fatigue machine TEKNIKER©, (b) thermal cracks reproduced in the tested* 

In the frame of the EU Project OPTIMIZE, TEKNIKER has upgraded the FZG machine, to measure the vibrations, noise, and transmission losses and to complement the study of micropitting, pitting, or scuffing phenomena (**Figure 20**). In this topic, the team has been working in the EU Projects TESS [33], OPTIMIZE

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

*5.2.4 Tribology of gears and transmissions*

**5.3 High-temperature tribology**

*drive motor intensity and (b) sensors and signals collected [34].*

*(PIM)*

**Figure 20.**

and SELENA.

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

### *5.2.4 Tribology of gears and transmissions*

In the frame of the EU Project OPTIMIZE, TEKNIKER has upgraded the FZG machine, to measure the vibrations, noise, and transmission losses and to complement the study of micropitting, pitting, or scuffing phenomena (**Figure 20**). In this topic, the team has been working in the EU Projects TESS [33], OPTIMIZE [34], EREBIO [35–37], VOSOLUB [38], SUNOIL [39], LUBRICOAT [40], BIOGREASE [39], and BIOMON [41] and the industrial projects AEROHUMs and SELENA.


### **Figure 20.**

*Friction, Lubrication and Wear*

**Coating type Load-**

**TiN + C (C sputtered)**

**Table 1.**

FALEX tribological test (Project BIOMON).

**carrying capacity**

*5.2.3 Tribology of clutches and brakes*

Industrial Project I-SINTER (clutches).

configuration to study the tribology of real bearings has been developed, adapted to

**Adherence Wear** 

CrN Good Good Good Medium Bad Mo Good Good Bad Low Bad TiAlN Good Medium–good Good High Good TiCN Bad-medium Bad Good High Good TiAlCN Medium Medium Good High Good

**Medium–good Good Medium–**

*Qualitative behavior of coatings to increase lifetime of rolling bearings [19].*

**protection**

**good**

**Hardness Fatigue** 

**Medium– high**

**resistance**

**Very good**

Brakes and clutches require high stable friction coefficient. To understand the tribology phenomena of these systems, testing protocols have been developed for the standard FALEX (high-performance and multispecimen) tribometers to study the friction wear mechanism of brakes and clutches (high temperature abrasion, adhesion, and fading) and to study the relationship of the friction coefficient with the squeal generation. Additionally, a dynamometer test bench has been constructed to test disc brakes (**Figure 9**) and clutches (**Figure 10**). In the frame of the i-SINTER Project, the correlation between the friction measured in pin on disc tests and the torque measured in clutch tests has been studied, observing very similar values, especially at low loads (**Figure 19**). These conditions were selected for screening of the materials with pin on disc tests, before final validation in the clutch test. The tribological knowledge on dry friction has been used in the projects M-eranet JOLIE (brakes) [21], Manunet BRAKE SQUEAL (clutches) [22], and

*Coefficient of friction during clutch test and pin on disc test carried out with the same materials.*

**162**

**Figure 19.**

*a) Upgrading of FZG machine to monitor vibration, transmission error, power losses, noise, temperature, and drive motor intensity and (b) sensors and signals collected [34].*

### **5.3 High-temperature tribology**

### *5.3.1 Tribology of high-pressure die casting (HPDC) and polymer injection molds (PIM)*

In the frame of MUSIC Project, a thermal fatigue machine has been constructed to reproduce the main failure of the high-pressure die casting molds. In **Figure 21a**, the thermal cycles can be seen in high-pressure die casting process reproduced in the thermal fatigue machine, and in **Figure 21b**, the thermal fatigue mechanism can be observed, reproduced in a flat specimen with internal cooling circuits, representing the die. The thermal fatigue mechanism can also be reproduced in 3D complex geometries. Setup of testing protocols has been carried out to simulate also other failure mechanisms of HPDC and PIM molds such as mechanical and chemical die soldering, abrasion and erosion resistance, and the corrosion behavior. The knowledge generated in MUSIC project has been applied to the EUROSTAR Project

### **Figure 21.**

*(a) Thermal cycles in the thermal fatigue machine TEKNIKER©, (b) thermal cracks reproduced in the tested block of the mold material after 10,000 thermal cycles.*

SUPERSLIP (to select surface treatments for polymer injection molds) and to the industrial projects HARCO, ALEPRE, MEFOLUB and MMPUL [20, 42–45].

### *5.3.2 Tribology of engine and turbine components*

The development of testing configurations adapted to standard tribological testing machines can be highlighted in order to test real parts of engine and turbine components (e.g., valve/guide contact, piston ring/cylinder liner contact, the piston skirt/cylinder liner contact, valve head/valve inserts, gudgeon pin/ piston, gland/piston rod, piston rod/seal, turbine support, etc.). In **Figure 22**, the results of scuffing tests of the piston ring/cylinder liner used to screen suitable biodegradable oils compatible with bioethanol for two stroke engine oils can be seen. Most of the lubricants suffered scuffing, except the one called SEMO36 that was suitable for the application. The testing protocols developed has been used in the EU Projects POWERFUL [46], EREBIO [47, 48], Nano-HVOF [49], EFCAP [50], COST [51], CLEANENGINE [52, 53], NANOMAG, and NADIA [32]; in the regional project TRIBORE and MOTOLURE [47]; in the industrial projects REMTRAL [51], AUMORE, RECOLURE, EQUIMOTOR and EQUIMOTOR PLUS [54], ABADIE, and 2 MW engine; and in the national projects RAMPE and ALELLA.

### **Figure 22.**

*(a) Piston ring/cylinder liner configuration developed by TEKNIKER. (b) Selection of SEMO 36 oil to avoid scuffing of bioethanol/biolubricant mixture, in piston ring/cylinder liner tests.*

### **5.4 Tribology of special materials**

### *5.4.1 Tribology of seals and elastomers*

As already described (see **Figure 11**), a test bench has been constructed to test real seals to study their friction, wear, and leakage under oscillatory and reciprocal motions. A simplified tribological test has also been developed to reproduce the failure mechanism and the friction and wear of the seals. In the frame of EU Project KRISTAL, the laser texturing was applied by TEKNIKER directly on seals materials or transferred through the molds. In **Figure 23a**, it can be observed the effect of surface laser texturing on seals materials reducing significantly the friction coefficient. In the EU project STOKES, different surface texturing geometries

**165**

**Figure 24.**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

were tested in the seals test bench constructed by TEKNIKER, selecting also the most appropriate texturing geometry. This knowledge has been applied to EU Projects FUNDTRIBO [26], ISSELUB, the regional projects MODELOST [23] and

In this context a test protocol has been developed to evaluate the friction (static and dynamic) and wear of the floorings determining the anti-slippery properties simulating the lifetime of the floor (**Figure 24**). This knowledge has been used in the national project TRIBOSTAND, in the EU Project SLIP SAFE, and in a regional

*(a) Effect of texturing to improve the tribological properties of different types of seals. (b) Results of the TESSA seal test bench TEKNIKER© with different texturing geometries and selection of the one reaching a* 

Testing protocols have been set up to evaluate mechanical properties, abrasion, and tactile properties of the textiles (**Figure 25**). This knowledge has been used in

*Test protocols have been developed to evaluate the durability, the cleanliness, and the comfort of the floorings* 

*(a) involving persons, (b) tribometers, and (c) contact angle measurements.*

EMAITEK [24, 25], and the industrial projects 3D FLEX and ELASWEAR.

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

*5.4.2 Tribology of anti-slippery floorings*

project SEGURPAV [55].

**Figure 23.**

*minimum torque.*

*5.4.3 Tribology of textiles*

the EU Project 2B FUNTEX [56].

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

were tested in the seals test bench constructed by TEKNIKER, selecting also the most appropriate texturing geometry. This knowledge has been applied to EU Projects FUNDTRIBO [26], ISSELUB, the regional projects MODELOST [23] and EMAITEK [24, 25], and the industrial projects 3D FLEX and ELASWEAR.

### **Figure 23.**

*Friction, Lubrication and Wear*

ALELLA.

**Figure 22.**

**5.4 Tribology of special materials**

*5.4.1 Tribology of seals and elastomers*

*5.3.2 Tribology of engine and turbine components*

SUPERSLIP (to select surface treatments for polymer injection molds) and to the industrial projects HARCO, ALEPRE, MEFOLUB and MMPUL [20, 42–45].

The development of testing configurations adapted to standard tribological testing machines can be highlighted in order to test real parts of engine and turbine components (e.g., valve/guide contact, piston ring/cylinder liner contact, the piston skirt/cylinder liner contact, valve head/valve inserts, gudgeon pin/ piston, gland/piston rod, piston rod/seal, turbine support, etc.). In **Figure 22**, the results of scuffing tests of the piston ring/cylinder liner used to screen suitable biodegradable oils compatible with bioethanol for two stroke engine oils can be seen. Most of the lubricants suffered scuffing, except the one called SEMO36 that was suitable for the application. The testing protocols developed has been used in the EU Projects POWERFUL [46], EREBIO [47, 48], Nano-HVOF [49], EFCAP [50], COST [51], CLEANENGINE [52, 53], NANOMAG, and NADIA [32]; in the regional project TRIBORE and MOTOLURE [47]; in the industrial projects REMTRAL [51], AUMORE, RECOLURE, EQUIMOTOR and EQUIMOTOR PLUS [54], ABADIE, and 2 MW engine; and in the national projects RAMPE and

As already described (see **Figure 11**), a test bench has been constructed to test real seals to study their friction, wear, and leakage under oscillatory and reciprocal motions. A simplified tribological test has also been developed to reproduce the failure mechanism and the friction and wear of the seals. In the frame of EU Project KRISTAL, the laser texturing was applied by TEKNIKER directly on seals materials or transferred through the molds. In **Figure 23a**, it can be observed the effect of surface laser texturing on seals materials reducing significantly the friction coefficient. In the EU project STOKES, different surface texturing geometries

*(a) Piston ring/cylinder liner configuration developed by TEKNIKER. (b) Selection of SEMO 36 oil to avoid* 

*scuffing of bioethanol/biolubricant mixture, in piston ring/cylinder liner tests.*

**164**

*(a) Effect of texturing to improve the tribological properties of different types of seals. (b) Results of the TESSA seal test bench TEKNIKER© with different texturing geometries and selection of the one reaching a minimum torque.*

### *5.4.2 Tribology of anti-slippery floorings*

In this context a test protocol has been developed to evaluate the friction (static and dynamic) and wear of the floorings determining the anti-slippery properties simulating the lifetime of the floor (**Figure 24**). This knowledge has been used in the national project TRIBOSTAND, in the EU Project SLIP SAFE, and in a regional project SEGURPAV [55].

**Figure 24.**

*Test protocols have been developed to evaluate the durability, the cleanliness, and the comfort of the floorings (a) involving persons, (b) tribometers, and (c) contact angle measurements.*

### *5.4.3 Tribology of textiles*

Testing protocols have been set up to evaluate mechanical properties, abrasion, and tactile properties of the textiles (**Figure 25**). This knowledge has been used in the EU Project 2B FUNTEX [56].

**Figure 25.**

*(a) Friction measurements as indicator of textile tactility in dry and wet conditions for cotton, polyester, and the 50% mixture. (b) Material used to simulate the skin at laboratory. (c) Real skin.*

### **5.5 Biotribology**

### *5.5.1 Tribology of autologous bones*

The use of impact and compression tests to understand the effect of thermal treatments in artificial bones and inserts has been studied in the frame of the EU Project AUTOBONE. In **Figure 26**, it can be appreciated that the thermal treatment reduces the wear caused by the impact, improving the toughness of the artificial inserts composed of hydroxyapatite and collagen [57].


### **Figure 26.**

*(a) Configuration of impact test. (b) Impact resistance of the hydroxyapatite/collagen bone inserts with and without thermal treatments.*

**167**

**Figure 27.**

*5.5.3 Dental tribology*

*with a top silver layer.*

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

A testing configuration has been designed adapted to a commercial FALEX tribometer to simulate the wear of hip/acetabular cup. Friction, wear, and tribocorrosion protocols have also been developed to simulate the lifetime of the hip and knee prosthesis. In **Figure 27**, it is possible to see how the TiCN-2 coating deposited by Physical vapor deposition (PVD) by TEKNIKER can enhance the tribocorrosion properties and antibacterial properties. The antibacterial properties are still enhanced when adding a sacrificial silver top layer, also applied by PVD. The Ag layer might be active as anti-infection layer, during implantation, since it will be easily removed due to their poor wear resistance. The protocols have been used in the national projects FUNCOAT, DELECA, SINOVIAL, FUNMAT in the industrial

The development of testing protocols can be highlighted to simulate friction, wear, impact, and tribocorrosion in dental implants. In **Figure 28**, the results of

*(a) Program for coating evaluation. (b) Tribocorrosion resistance of Ti6Al4V alloy before and after coating with TiCN-1 and TiCN-2. (c) Antibacterial properties of Ti6Al4V, after coating with TiCN-2 without and* 

BIOTIDE project, and the Eurostars INNOVATIDE Project [29–31].

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

*5.5.2 Tribology of hip and knee implants*

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

### *5.5.2 Tribology of hip and knee implants*

*Friction, Lubrication and Wear*

**166**

**Figure 26.**

*without thermal treatments.*

**5.5 Biotribology**

**Figure 25.**

*5.5.1 Tribology of autologous bones*

composed of hydroxyapatite and collagen [57].

The use of impact and compression tests to understand the effect of thermal treatments in artificial bones and inserts has been studied in the frame of the EU Project AUTOBONE. In **Figure 26**, it can be appreciated that the thermal treatment reduces the wear caused by the impact, improving the toughness of the artificial inserts

*(a) Friction measurements as indicator of textile tactility in dry and wet conditions for cotton, polyester, and* 

*the 50% mixture. (b) Material used to simulate the skin at laboratory. (c) Real skin.*

*(a) Configuration of impact test. (b) Impact resistance of the hydroxyapatite/collagen bone inserts with and* 

A testing configuration has been designed adapted to a commercial FALEX tribometer to simulate the wear of hip/acetabular cup. Friction, wear, and tribocorrosion protocols have also been developed to simulate the lifetime of the hip and knee prosthesis. In **Figure 27**, it is possible to see how the TiCN-2 coating deposited by Physical vapor deposition (PVD) by TEKNIKER can enhance the tribocorrosion properties and antibacterial properties. The antibacterial properties are still enhanced when adding a sacrificial silver top layer, also applied by PVD. The Ag layer might be active as anti-infection layer, during implantation, since it will be easily removed due to their poor wear resistance. The protocols have been used in the national projects FUNCOAT, DELECA, SINOVIAL, FUNMAT in the industrial BIOTIDE project, and the Eurostars INNOVATIDE Project [29–31].

### **Figure 27.**

*(a) Program for coating evaluation. (b) Tribocorrosion resistance of Ti6Al4V alloy before and after coating with TiCN-1 and TiCN-2. (c) Antibacterial properties of Ti6Al4V, after coating with TiCN-2 without and with a top silver layer.*

### *5.5.3 Dental tribology*

The development of testing protocols can be highlighted to simulate friction, wear, impact, and tribocorrosion in dental implants. In **Figure 28**, the results of

tribocorrosion tests carried out to compare the behavior of titanium before and after treatment with different plasma electrooxidation coatings (PEO) developed by TEKNIKER using different process conditions are represented. The behavior of the coatings improved when increasing the plasma intensity. Also, the wear volume of a reference and new electrolyte was compared observing a significative improvement with the new electrolyte developed in TEKNIKER. This knowledge has been applied to the national project FUNCOAT and industrial projects [58].

### **Figure 28.**

*(a) Tribocorrosion test of titanium (Ti) coated with two types of PEO coatings. (b) Wear volume of tribocorrosion test of Ti and PEO coatings using two electrolytes.*

### *5.5.4 Tactile properties of steel*

A similar test protocol mentioned in Section 5.4.3 has also been used to evaluate the steel sheet tactility. The effect of the textured surface geometries of steel sheet surfaces transferred by lamination with laser textured rollers has been studied. The laser texturing was carried out by TEKNIKER. This knowledge has been used in the EU Project STEELTAC [59].

### **5.6 Tribolubrication**

### *5.6.1 Tribology of environmentally friendly lubricants for cutting and forming applications*

Testing protocols has been developed to compare tapping torque results and center of numeric control (CNC) machines to screen torque and wear of cutting and forming fluids and different coatings to increase the efficiency. In the EU

### **Figure 29.**

*Comparison of mineral and vegetable lubricants measuring (a) relative efficiency in tapping torque machine and (b) flank wear in CNC grinding machine.*

**169**

**Figure 31.**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

Project VOSOLUB [60], similar tribological properties have been shown between mineral- and vegetable-based cutting lubricants. Both the efficiency of the fluids measuring the torque with the tapping torque machine and the flank wear with a CNC controlled grinding machine have been evaluated (**Figure 29**). The knowledge has been applied to EU Projects IBIOLAB [60], DECOLUB [61], and other related projects such as ECOLUBRO, NANOCOMP, MEFOLUB, and CLAREFOSS.

Testing protocols have been developed to compare the behavior of the biolubricants as alternative to mineral-based oils to lubricate mechanical components (e.g., wind mills, hydraulic pumps, excavators). In the example, a glycol-free lubricant has been developed increasing their load-carrying capacity in comparison with the glycol-containing one. The glycol-free lubricant is biodegradable, and it can be an interesting alternative as a fire-resistant hydraulic oil (**Figure 30**). The protocols have been used in the EU Projects VOSOLUB [38], SUNOIL and BIOGREASE, [39], LUBRICOAT [40], CTVO-NET and LLINCWA [62], BIOMON and IBIOLAB [41], the national projects LUVE and BIOVESIN [63, 64], and the industrial projects ADIVINA, PAVIA, and NANOINTECH.

Testing protocols has been developed also to evaluate the behavior of ionic liquids as lubricants in different environments studying friction, wear, and tribocorrosion behavior. In **Figure 31**, it is represented the friction and wear scar of the Ionic Liquids DIL3 and

*(a) Load-carrying capacity of glycol and glycol-free lubricants. (b) Biodegradability of glycol-free lubricants >60%.*

*In the figure, the friction and wear scar of the ionic liquids DIL3 and DIL7, patented by TEKNIKER, are* 

*compared with the hybrid ionic liquid synthetized by TEKNIKER.*

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

*5.6.3 Tribology of ionic liquids*

**Figure 30.**

*5.6.2 Tribology of biolubricants for bearings and gears*

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

Project VOSOLUB [60], similar tribological properties have been shown between mineral- and vegetable-based cutting lubricants. Both the efficiency of the fluids measuring the torque with the tapping torque machine and the flank wear with a CNC controlled grinding machine have been evaluated (**Figure 29**). The knowledge has been applied to EU Projects IBIOLAB [60], DECOLUB [61], and other related projects such as ECOLUBRO, NANOCOMP, MEFOLUB, and CLAREFOSS.

### *5.6.2 Tribology of biolubricants for bearings and gears*

Testing protocols have been developed to compare the behavior of the biolubricants as alternative to mineral-based oils to lubricate mechanical components (e.g., wind mills, hydraulic pumps, excavators). In the example, a glycol-free lubricant has been developed increasing their load-carrying capacity in comparison with the glycol-containing one. The glycol-free lubricant is biodegradable, and it can be an interesting alternative as a fire-resistant hydraulic oil (**Figure 30**). The protocols have been used in the EU Projects VOSOLUB [38], SUNOIL and BIOGREASE, [39], LUBRICOAT [40], CTVO-NET and LLINCWA [62], BIOMON and IBIOLAB [41], the national projects LUVE and BIOVESIN [63, 64], and the industrial projects ADIVINA, PAVIA, and NANOINTECH.

### **Figure 30.**

*Friction, Lubrication and Wear*

*5.5.4 Tactile properties of steel*

*tribocorrosion test of Ti and PEO coatings using two electrolytes.*

**Figure 28.**

EU Project STEELTAC [59].

**5.6 Tribolubrication**

*applications*

tribocorrosion tests carried out to compare the behavior of titanium before and after treatment with different plasma electrooxidation coatings (PEO) developed by TEKNIKER using different process conditions are represented. The behavior of the coatings improved when increasing the plasma intensity. Also, the wear volume of a reference and new electrolyte was compared observing a significative improvement with the new electrolyte developed in TEKNIKER. This knowledge has been applied to the national project FUNCOAT and industrial projects [58].

A similar test protocol mentioned in Section 5.4.3 has also been used to evaluate the steel sheet tactility. The effect of the textured surface geometries of steel sheet surfaces transferred by lamination with laser textured rollers has been studied. The laser texturing was carried out by TEKNIKER. This knowledge has been used in the

*5.6.1 Tribology of environmentally friendly lubricants for cutting and forming* 

*(a) Tribocorrosion test of titanium (Ti) coated with two types of PEO coatings. (b) Wear volume of* 

Testing protocols has been developed to compare tapping torque results and center of numeric control (CNC) machines to screen torque and wear of cutting and forming fluids and different coatings to increase the efficiency. In the EU

*Comparison of mineral and vegetable lubricants measuring (a) relative efficiency in tapping torque machine* 

**168**

**Figure 29.**

*and (b) flank wear in CNC grinding machine.*

*(a) Load-carrying capacity of glycol and glycol-free lubricants. (b) Biodegradability of glycol-free lubricants >60%.*

### *5.6.3 Tribology of ionic liquids*

Testing protocols has been developed also to evaluate the behavior of ionic liquids as lubricants in different environments studying friction, wear, and tribocorrosion behavior. In **Figure 31**, it is represented the friction and wear scar of the Ionic Liquids DIL3 and

### **Figure 31.**

*In the figure, the friction and wear scar of the ionic liquids DIL3 and DIL7, patented by TEKNIKER, are compared with the hybrid ionic liquid synthetized by TEKNIKER.*

DIL7, patented by TEKNIKER (EFS/ID/12720945) and developed in the frame of EU Project MINILUBES Project has been compared with a hybrid ionic liquid synthetized by TEKNIKER, developed in the EMAITEK project, are represented. In this subject, the activity carried out in Eurostar Project VACUUM DLC, the EMAITEK Basque Country Initiative, and the Austrian COMET Project can be also mentioned [65–67].

### **5.7 Tribology of materials for energy**

### *5.7.1 Tribology for biogas, biodiesel, and bioethanol*

Testing protocols has been set up to determine the durability of fuel injectors and other critical engine components of engines working with biogas or suffering lubricant dilution with biodiesel, bioethanol, or their mixtures. In **Figure 32**, it is represented the friction coefficient of the PVD coating Ti-DLC coating deposited by TEKNIKER on injectors, comparing the behavior between diesel and biodiesel (B50, 50% diesel and 50% biodiesel). The protocols have been used in the EU Project Cleanengine and in the industrial project IDEA [68].

### **Figure 32.**

*(a) Tribological properties of the Ti-DLC coating, simulating the contact of injector nozzles with diesel and biodiesel B50; and (b) testing configuration.*

### *5.7.2 Tribology in energy-efficient systems*

Testing protocols have been set up to compare the lifetime of critical components of heat exchangers, compressors, gensets, and microturbines. In the example,

### **Figure 33.**

*Average main torque obtained with the drag friction test with different heat exchange fluids of different viscosities (mPa). Error bars represent average standard deviation.*

**171**

results.

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

the drag friction test developed by TEKNIKER (**Figure 3**), has been used to evaluate the average torque of different heat exchanger fluids, named as HTF-800 and HTF-200. The last one was tested at different viscosities from 10 to 100 mPa s. The minimum torque was measured for the HT-800 fluid, being finally selected for the application in SUSPIRE Project (**Figure 33**). The protocols have been applied to EU

Attention to tribological problems would imply worldwide annual savings of 970,000 M€ (1.39% GDP) [69]. A huge range of new testing equipment and protocols have been developed to simulate the friction and wear (mechanical and chemical) of a wide range of mechanical components and systems, in different environments. The knowledge about the working conditions and the failure mechanisms will make possible in the future to simulate at laboratory a still wider list of tribological systems. This will also help us to make a step forward, toward modeling the extrapolation of research results to real systems and the generation of new standards. Artificial intelligence can be also a tool that can facilitate this step forward. Tribology will help to design low carbon footprint materials and implement them in a cost-efficient, predictive, and safe way [70–75]. Tribology will assist also the development of energy- and resource-efficient products and processes, in

The authors acknowledge the financing from the European Commission, the Spanish Minister of Science and Technology and CDTI, the Basque Country Government SPRI and InnoBasque, the Gipuzkoa Provincial Council and the X-Tribology Austrian COMET Program. The authors also acknowledge the cooperation and/or financing of the industries and research institutions participating in each project. The authors made special mention to those members of the tribology team, that completed their Doctoral Thesis for their contribution to the knowledge generated: Bihotz Pinedo (Tribology of seals 2016) [23-25, 27], Borja Zabala (high Temperature Tribology (eg. moulds, engines) 2017) [20, 22, 42, 43, 46, 52], Francesco Pagano, (tribology of ionic liquids and vacuum tribology, 2017) [2–4, 13, 57–65], Beatriz Fernandez-Diaz (tribology of polymers, 2017) [28, 34, 63], Virginia Saenz de Viteri (biotribology, 2016) [30, 31, 56, 57], Sofia Alves (dental tribology, 2017) [58], Cristina Cerrillo (ecotoxicity of nanoparticles, 2016) [71–75], Ainara López (marine and off shore tribology, 2018) [12–16]. Also, to all the members of the tribology team that dedicate their professional work to tribology activity Elena Fuentes [17, 18, 30, 40, 56, 57], Xana Fernandez [9, 11, 29, 31, 46–48, 54, 65], Gemma Mendoza [5, 11, 32, 49, 50, 60, 63, 71–73], Xanti Almandoz [34], Juan Carlos Rodriguez [8, 9, 16, 34], Olatz Areitioaurtena [48, 67, 68, 71–73], Marcello Conte [1, 2, 23–25, 27, 54], and Roman Nevshupa [1, 4, 7, 8, 46, 52, 54], and the other members of the research group that contributed to the generation of the

Project HEGEL [68] and to the industrial project ABADIE PLUS [69].

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

**6. Conclusions**

real systems.

**Acknowledgements**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

the drag friction test developed by TEKNIKER (**Figure 3**), has been used to evaluate the average torque of different heat exchanger fluids, named as HTF-800 and HTF-200. The last one was tested at different viscosities from 10 to 100 mPa s. The minimum torque was measured for the HT-800 fluid, being finally selected for the application in SUSPIRE Project (**Figure 33**). The protocols have been applied to EU Project HEGEL [68] and to the industrial project ABADIE PLUS [69].

### **6. Conclusions**

*Friction, Lubrication and Wear*

**5.7 Tribology of materials for energy**

*5.7.2 Tribology in energy-efficient systems*

*biodiesel B50; and (b) testing configuration.*

*5.7.1 Tribology for biogas, biodiesel, and bioethanol*

Project Cleanengine and in the industrial project IDEA [68].

DIL7, patented by TEKNIKER (EFS/ID/12720945) and developed in the frame of EU Project MINILUBES Project has been compared with a hybrid ionic liquid synthetized by TEKNIKER, developed in the EMAITEK project, are represented. In this subject, the activity carried out in Eurostar Project VACUUM DLC, the EMAITEK Basque Country

Testing protocols has been set up to determine the durability of fuel injectors and other critical engine components of engines working with biogas or suffering lubricant dilution with biodiesel, bioethanol, or their mixtures. In **Figure 32**, it is represented the friction coefficient of the PVD coating Ti-DLC coating deposited by TEKNIKER on injectors, comparing the behavior between diesel and biodiesel (B50, 50% diesel and 50% biodiesel). The protocols have been used in the EU

Testing protocols have been set up to compare the lifetime of critical components of heat exchangers, compressors, gensets, and microturbines. In the example,

*(a) Tribological properties of the Ti-DLC coating, simulating the contact of injector nozzles with diesel and* 

*Average main torque obtained with the drag friction test with different heat exchange fluids of different* 

*viscosities (mPa). Error bars represent average standard deviation.*

Initiative, and the Austrian COMET Project can be also mentioned [65–67].

**170**

**Figure 33.**

**Figure 32.**

Attention to tribological problems would imply worldwide annual savings of 970,000 M€ (1.39% GDP) [69]. A huge range of new testing equipment and protocols have been developed to simulate the friction and wear (mechanical and chemical) of a wide range of mechanical components and systems, in different environments. The knowledge about the working conditions and the failure mechanisms will make possible in the future to simulate at laboratory a still wider list of tribological systems. This will also help us to make a step forward, toward modeling the extrapolation of research results to real systems and the generation of new standards. Artificial intelligence can be also a tool that can facilitate this step forward. Tribology will help to design low carbon footprint materials and implement them in a cost-efficient, predictive, and safe way [70–75]. Tribology will assist also the development of energy- and resource-efficient products and processes, in real systems.

### **Acknowledgements**

The authors acknowledge the financing from the European Commission, the Spanish Minister of Science and Technology and CDTI, the Basque Country Government SPRI and InnoBasque, the Gipuzkoa Provincial Council and the X-Tribology Austrian COMET Program. The authors also acknowledge the cooperation and/or financing of the industries and research institutions participating in each project. The authors made special mention to those members of the tribology team, that completed their Doctoral Thesis for their contribution to the knowledge generated: Bihotz Pinedo (Tribology of seals 2016) [23-25, 27], Borja Zabala (high Temperature Tribology (eg. moulds, engines) 2017) [20, 22, 42, 43, 46, 52], Francesco Pagano, (tribology of ionic liquids and vacuum tribology, 2017) [2–4, 13, 57–65], Beatriz Fernandez-Diaz (tribology of polymers, 2017) [28, 34, 63], Virginia Saenz de Viteri (biotribology, 2016) [30, 31, 56, 57], Sofia Alves (dental tribology, 2017) [58], Cristina Cerrillo (ecotoxicity of nanoparticles, 2016) [71–75], Ainara López (marine and off shore tribology, 2018) [12–16]. Also, to all the members of the tribology team that dedicate their professional work to tribology activity Elena Fuentes [17, 18, 30, 40, 56, 57], Xana Fernandez [9, 11, 29, 31, 46–48, 54, 65], Gemma Mendoza [5, 11, 32, 49, 50, 60, 63, 71–73], Xanti Almandoz [34], Juan Carlos Rodriguez [8, 9, 16, 34], Olatz Areitioaurtena [48, 67, 68, 71–73], Marcello Conte [1, 2, 23–25, 27, 54], and Roman Nevshupa [1, 4, 7, 8, 46, 52, 54], and the other members of the research group that contributed to the generation of the results.

*Friction, Lubrication and Wear*

### **Author details**

Amaya Igartua1 \*, Raquel Bayon1 , Ana Aranzabe1 and Javier Laucirica<sup>2</sup>

1 Fundación TEKNIKER, Eibar, Spain

2 IK4, Eibar, Spain

\*Address all correspondence to: amaya.igartua@tekniker.es

A summary of 37 years' experience in TEKNIKER.

© 2019 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

**173**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

2010;**396**(8):2855-2862. DOI: 10.1007/

[8] Bayon R, Zubizarreta C, Nevshupa R, Rodríguez JC, Fernández X, Ruiz de Gurpegui U, et al. Rollingsliding, scuffing and tribocorrosion behaviour of PVD multilayer coatings for gear applications. Tribology International. 2011;**63**(1):17-26. DOI:

[9] Bayon R, Igartua A, Fernandez X, Martinez R, Rodriguez JC, Garcia JA, et al. Corrosion-wear behaviour of PVD Cr/CrN multilayer coatings for gear applications. Tribology International. 2009;**42**:591-599. DOI: 10.1016/j.

[10] Celis JP, Ponthiaux P, Bayón R, Igartua A. Testing Tribocorrosion of Passivating Materials Supporting Research and Industrial Innovation:

Publishing; 2012. European Federation

[11] Igartua A, Bayon R, Mendoza G, Fernandez X, Ciarsolo I, Aramburu E, et al. Corrosion and tribocorrosion studies on PVD coatings for aeronautical applications. In: Workshop on Surface Treatments and Coatings for Mechanical and Aeronautical Applications; 28-30

Handbook. London: Maney

of Corrosion. Available from: https://www.taylorfrancis.com/

books/e/9781351546942

Marzo 2007; Sevilla. 2007

10.1155/2018/7345346

[12] López-Ortega A, Arana JL, Bayón R. Tribocorrosion of passive materials: A review on test procedures and standards. International Journal of Corrosion. 2018;**1**:7345346. DOI:

[13] López A, Bayón R, Pagano F, Igartua A, Arredondo A, Arana JL, et al. Tribocorrosion behaviour of mooring high strength low alloy steels in synthetic seawater. Wear.

10.1108/00368791111101803

triboint.2008.06.015

s00216-010-3538-6

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

[1] Nevshupa A, Conte M, Igartua A, Roman E, Segovia JL. Ultrahigh vacuum system for advanced tribology studies: Design principles and applications. Tribology International. 2015;**86**:28-36. DOI: 10.1016/j.triboint.2015.01.020

[2] Totolin V, Conte M, Berriozabal E, Pagano F, Minami I, Dörr N, et al. Tribological investigation of ionic liquids in ultra-high vacuum environment. Lubrication Science. 2014;**26**:514-524. DOI: 10.1002/ls.1224

[3] Igartua A, Pagano F, Bayon R, Minami I, Doerr N. Ionic liquids in space applications. In: TAE Congress of Tribology; January 2018; Esslingen,

[4] Igartua A, Berriozabal E, Nevshupa R, Roman E, Pagano F, Pleth Nielsen L, et al. Screening of diamondlike carbon coatings in search of a prospective solid lubricant suitable for both atmosphere and high vacuum applications. Tribology International. 2017;**114**:192-200. DOI: 10.1016/j.

[5] Silva ER, Ferreira O, Ramalho PA, Azevedo NF, Bayon R, Igartua A, et al. Ecofriendly non biocide reléase coatings for marine biofouling prevention. Science of the Total Environment. 2019;**650**(2):2499-2511. DOI: 10.1016/j.

[6] Tulcidas AV, Bayon R, Igartua A, Bordado JMC, Silva ER. Friction reduction on recent non releasing biocidal coatings by a newly designed friction test rig. Tribology International.

2015;**91**:140-150. DOI: 10.1016/j.

[7] Bayón R, Nevshupa R, Zubizarreta C, Ruiz de Gopegui U, Barriga J, Igartua A. Characterisation of tribocorrosion behaviour of multilayer PVD coatings. Analytical and Bioanalytical Chemistry.

Germany. 2018

**References**

triboint.2017.04.024

scitotenv.2018.10.010

triboint.2015.06.017

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

### **References**

*Friction, Lubrication and Wear*

**172**

**Author details**

Amaya Igartua1

2 IK4, Eibar, Spain

provided the original work is properly cited.

\*, Raquel Bayon1

\*Address all correspondence to: amaya.igartua@tekniker.es

A summary of 37 years' experience in TEKNIKER.

1 Fundación TEKNIKER, Eibar, Spain

© 2019 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium,

, Ana Aranzabe1

and Javier Laucirica<sup>2</sup>

[1] Nevshupa A, Conte M, Igartua A, Roman E, Segovia JL. Ultrahigh vacuum system for advanced tribology studies: Design principles and applications. Tribology International. 2015;**86**:28-36. DOI: 10.1016/j.triboint.2015.01.020

[2] Totolin V, Conte M, Berriozabal E, Pagano F, Minami I, Dörr N, et al. Tribological investigation of ionic liquids in ultra-high vacuum environment. Lubrication Science. 2014;**26**:514-524. DOI: 10.1002/ls.1224

[3] Igartua A, Pagano F, Bayon R, Minami I, Doerr N. Ionic liquids in space applications. In: TAE Congress of Tribology; January 2018; Esslingen, Germany. 2018

[4] Igartua A, Berriozabal E, Nevshupa R, Roman E, Pagano F, Pleth Nielsen L, et al. Screening of diamondlike carbon coatings in search of a prospective solid lubricant suitable for both atmosphere and high vacuum applications. Tribology International. 2017;**114**:192-200. DOI: 10.1016/j. triboint.2017.04.024

[5] Silva ER, Ferreira O, Ramalho PA, Azevedo NF, Bayon R, Igartua A, et al. Ecofriendly non biocide reléase coatings for marine biofouling prevention. Science of the Total Environment. 2019;**650**(2):2499-2511. DOI: 10.1016/j. scitotenv.2018.10.010

[6] Tulcidas AV, Bayon R, Igartua A, Bordado JMC, Silva ER. Friction reduction on recent non releasing biocidal coatings by a newly designed friction test rig. Tribology International. 2015;**91**:140-150. DOI: 10.1016/j. triboint.2015.06.017

[7] Bayón R, Nevshupa R, Zubizarreta C, Ruiz de Gopegui U, Barriga J, Igartua A. Characterisation of tribocorrosion behaviour of multilayer PVD coatings. Analytical and Bioanalytical Chemistry. 2010;**396**(8):2855-2862. DOI: 10.1007/ s00216-010-3538-6

[8] Bayon R, Zubizarreta C, Nevshupa R, Rodríguez JC, Fernández X, Ruiz de Gurpegui U, et al. Rollingsliding, scuffing and tribocorrosion behaviour of PVD multilayer coatings for gear applications. Tribology International. 2011;**63**(1):17-26. DOI: 10.1108/00368791111101803

[9] Bayon R, Igartua A, Fernandez X, Martinez R, Rodriguez JC, Garcia JA, et al. Corrosion-wear behaviour of PVD Cr/CrN multilayer coatings for gear applications. Tribology International. 2009;**42**:591-599. DOI: 10.1016/j. triboint.2008.06.015

[10] Celis JP, Ponthiaux P, Bayón R, Igartua A. Testing Tribocorrosion of Passivating Materials Supporting Research and Industrial Innovation: Handbook. London: Maney Publishing; 2012. European Federation of Corrosion. Available from: https://www.taylorfrancis.com/ books/e/9781351546942

[11] Igartua A, Bayon R, Mendoza G, Fernandez X, Ciarsolo I, Aramburu E, et al. Corrosion and tribocorrosion studies on PVD coatings for aeronautical applications. In: Workshop on Surface Treatments and Coatings for Mechanical and Aeronautical Applications; 28-30 Marzo 2007; Sevilla. 2007

[12] López-Ortega A, Arana JL, Bayón R. Tribocorrosion of passive materials: A review on test procedures and standards. International Journal of Corrosion. 2018;**1**:7345346. DOI: 10.1155/2018/7345346

[13] López A, Bayón R, Pagano F, Igartua A, Arredondo A, Arana JL, et al. Tribocorrosion behaviour of mooring high strength low alloy steels in synthetic seawater. Wear.

2015;**338-339**:1-10. DOI: 10.1016/j. wear.2015.05.004

[14] López-Ortega A, Bayón R, Arana JL, Arredondo A, Igartua A. Influence of temperature on the corrosion and tribocorrosion behaviour of high strength low alloy steels used in offshore applications. Tribology International. 2018;**121**:341-352. DOI: 10.1016/j. wear.2015.05.00

[15] López-Ortega A, Bayón R, Arana JL. Evaluation of protective coatings for offshore applications. Corrosion and tribocorrosion behavior in synthetic seawater. Surface & Coatings Technology. 2018;**349**:1083-1097. DOI: 10.1016/j.surfcoat.2018.06.089

[16] López-Ortega A, Arana JL, Rodríguez E, Bayón R. Corrosion, wear and tribocorrosion performance of a thermally sprayed aluminum coating modified by plasma electrolytic oxidation for offshore submerged components protection. Corrosion Science. 2018;**143**:258-280. DOI: 10.1016/j.corsci.2018.08.001

[17] Fuentes E, Kanase K. Friction and wear in engine bearings. In: Critical Component Wear in Heavy Duty Engines. Singapore: John Wiley & Sons; 2011. DOI: 10.1002/978047082 8847. ch12. ISBN 978-0-470-82882-3

[18] Kallio M, Vuorinen P, Fuentes E, Maraña O, Ruusila V, Nyysönnen T, et al. Tribological behaviour of bronze alloys with solid lubricants. Key Engineering Materials. 2013;**527**:205-210

[19] Igartua A, Laucirica J, Aranzabe A. Application of low temperature PVD coatings in rolling bearings. Tribological tests and experiences with spindle bearing systems. Surface and Coating Technology. 1996;**1**:460-467. DOI: 10.1016/ S0257-8972(96)03050-2

[20] Zabala B. Doctoral thesis. Universidad País Vasco; 2017

[21] Gorjan L, Boretius M, Guglan G, Kuebler J, Igartua A. Ceramic protection plates brazed to aluminum brake discs. Ceramics International. 2016;**42**(14):15739-15746. DOI: 10.1016/j.ceramint.2016.07.035

[22] Zarraga O, Abete JM, Ulacia I, Zabala B, Uzkudun O. On the Development of a Simple Model of a Brake Clutch for Squeal Prediction, Congress Eurobrake. 2014. pp. 13-14

[23] Pinedo B, Aguirrebeitia J, Conte M, Igartua A. Tri-dimensional eccentricity model of a rod lip seal. Tribology International. 2014;**78**:68-74. DOI: 10.1016/j.triboint.2014.05.005

[24] Conte M, Pinedo B, Igartua A. Frictional heating calculation based on tailored experimental measurements. Tribology International. 2014;**74**:1-6. DOI: 10.1016/j.triboint.2014.01.020

[25] Conte M, Pinedo B, Igartua A. Role of crystallinity on wear behaviour of PTFE composites. Wear. 2013;**307**: 81-86. DOI: 10.1016/j.wear.2013.08.019

[26] Lin LY, Tlatlik H, Gralla R, Igartua A, Baets P, Schlarb AK. Mechanical and thermal behaviors of polyether etherketone-based multi-scale composites. Journal of Composite Materials. 2012;**2**(10):1-18. DOI: 10.1177/0021998312454317

[27] Pinedo B, Hadfield M, Tzanakis I, Conte M, Anand M. Thermal analysis and tribological investigation on TPU and NBR elastomers applied to sealing applications. Tribology International. 2018;**127**:24-36. DOI: 10.1016/j. triboint.2018.05.032

[28] Fernandez B. Tesis doctoral; Universidad del País Vasco; 2017

[29] Saenz de Viteri V, Barandika G, Bayon R, Fernandez X, Ciarsolo I, Igartua A, et al. Development of Ti-C-N coatings with improved

**175**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

2008;**42**(1):77-87. DOI: 10.1016/j.

[37] Martins RC, Cardoso NFR, Bock H, Igartua A, Seabra JHO. Power loss performance of high pressure nitrided steel gears. Tribology International. 2009;**42**:1807-1815. DOI: 10.1016/j.

[38] Leao JD, Bouillon V, Muntada L, Johnson C, Wilson P, Vergnes O, et al. New formulations of sunflower based bio-lubricants with high oleic acid content. Oilseeds and fats, Crops and Lipids. 2016;**23**(5):D509. DOI: 10.1051/

[39] Igartua A, Barriga J, Aranzabe A. Biodegradable Lubricants. Vol. 1. Radom, Poland: Virtual Tribological Institute; 2005. pp. I.1-VI.3. ISBN 83-7204-449-X

[40] Vercammen K, Van Acker K, Barriga J, Fuentes E, Kalin M, Vizintin J. Combining biolubricants and low friction coatings. In: Current Trends in Tribology. Vol. I. Poland: ITEE; 2005.

pp. 1-4. ISBN 83-70204-418-X

[41] Igartua A. Biolubricants & their control for sustainable developments. Lube. 2007;**81**:6. ISSN 1744-5418

[42] Zabala B, Igartua A, Scarpi V, Timelli G, Girot F. Multiparametric study of Leidenfrost point and wettability of lubricants on highpressure die-casting dies. International

Journal of Thermal Sciences. 2018;**125**:66-73. DOI: 10.1016/j. ijthermalsci.2017.11.014

[43] Zabala B, Igartua A, Raone C, Timelli G, Bonollo F, Scarpi V, Peggiato

M, Girot F, "Evaluation HPDC Lubricant Spraying for Improved Cooling and Die Protection, LUBMAT Conference, 2016. Available from: https://www.researchgate.net/ publication/315837772\_Evaluation\_ HPDC\_Lubricant\_Spraying\_for\_ Improved\_Cooling\_and\_Die\_Protection

triboint. 2008.05.010

triboint.2009.03.006

ocl/2016033

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

tribological behavior and antibacterial properties. Journal of the Mechanical Behavior of Biomedical Materials. 2016;**55**:75-86. DOI: 10.1016/j.

jmbbm.2015.10.020

DOI: 10.5772/55860

[30] Sáenz de Viteri V, Fuentes E. Titanium and Titanium Alloys as Biomaterials. Rijeka, Croatia: InTech.

10.1016/j.apsusc.2016.01.145

Sviluppo. 2014;**67**:44-52

361992. pp. 54-61

[32] Igartua A, Bayon R, Mendoza G. Plasma electrolytic oxidation coatings for engine components. Ricerca e

[33] Laucirica J, Arnaiz A, Igartua A. Mantenimiento y control mediante Sistema experto; Forum Calidad. Vol.

[34] Presa J, Fernández-Díaz B, Igartua A, San José E, Almandoz X, Rodríguez JC, et al. Effects of manufacturing errors in the behaviour of a power gearbox. In: LUBMAT Conference; June 2016. 2016. Available from: https:// www.slideshare.net/TogetherToSolve/ effects-of-manufacturing-errors-in-the-

behaviour-of-a-power-gearbox

[35] Martins R, Seabra J, Brito A, Seyfert C, Luther R, Igartua A. Friction coefficient in FZG gears lubricated with industrial gear oils: Biodegradable ester vs. mineral oil. Tribology International.

2006;**39**:512-521. DOI: 10.1016/j.

[36] Cardoso NFR, Martins RC, Seabra JHO, Igartua A, Rodriguez JC, Luther R. Micropitting performance of nitrided steel gears lubricated with mineral and ester oils. Tribology International.

triboint.2005.03.021

[31] Sáenz de Viteri V, Bayon R, Igartua A, Barandika G, Moreno JE, Pérez C, et al. Structure, tribocorrosion and biocide characterization of Ca, P and I containing TiO2 coatings developed by plasma electrolytic oxidation. Applied Surface Science. 2016;**367**:1-10. DOI:

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

tribological behavior and antibacterial properties. Journal of the Mechanical Behavior of Biomedical Materials. 2016;**55**:75-86. DOI: 10.1016/j. jmbbm.2015.10.020

*Friction, Lubrication and Wear*

wear.2015.05.004

wear.2015.05.00

2015;**338-339**:1-10. DOI: 10.1016/j.

[21] Gorjan L, Boretius M, Guglan G, Kuebler J, Igartua A. Ceramic protection plates brazed to aluminum brake discs. Ceramics International. 2016;**42**(14):15739-15746. DOI: 10.1016/j.ceramint.2016.07.035

[22] Zarraga O, Abete JM, Ulacia I, Zabala B, Uzkudun O. On the Development of a Simple Model of a Brake Clutch for Squeal Prediction, Congress Eurobrake. 2014. pp. 13-14

[24] Conte M, Pinedo B, Igartua A. Frictional heating calculation based on tailored experimental measurements. Tribology International. 2014;**74**:1-6. DOI: 10.1016/j.triboint.2014.01.020

[23] Pinedo B, Aguirrebeitia J, Conte M, Igartua A. Tri-dimensional eccentricity model of a rod lip seal. Tribology International. 2014;**78**:68-74. DOI: 10.1016/j.triboint.2014.05.005

[25] Conte M, Pinedo B, Igartua A. Role of crystallinity on wear behaviour of PTFE composites. Wear. 2013;**307**: 81-86. DOI: 10.1016/j.wear.2013.08.019

[26] Lin LY, Tlatlik H, Gralla R, Igartua A, Baets P, Schlarb AK. Mechanical and thermal behaviors of polyether etherketone-based multi-scale composites. Journal of Composite Materials. 2012;**2**(10):1-18. DOI: 10.1177/0021998312454317

[27] Pinedo B, Hadfield M, Tzanakis I, Conte M, Anand M. Thermal analysis and tribological investigation on TPU and NBR elastomers applied to sealing applications. Tribology International. 2018;**127**:24-36. DOI: 10.1016/j.

[28] Fernandez B. Tesis doctoral; Universidad del País Vasco; 2017

[29] Saenz de Viteri V, Barandika G, Bayon R, Fernandez X, Ciarsolo I, Igartua A, et al. Development of Ti-C-N coatings with improved

triboint.2018.05.032

[14] López-Ortega A, Bayón R, Arana JL, Arredondo A, Igartua A. Influence of temperature on the corrosion and tribocorrosion behaviour of high

strength low alloy steels used in offshore applications. Tribology International. 2018;**121**:341-352. DOI: 10.1016/j.

[15] López-Ortega A, Bayón R, Arana JL. Evaluation of protective coatings for offshore applications. Corrosion and tribocorrosion behavior in

synthetic seawater. Surface & Coatings Technology. 2018;**349**:1083-1097. DOI:

[17] Fuentes E, Kanase K. Friction and wear in engine bearings. In: Critical Component Wear in Heavy Duty Engines. Singapore: John Wiley & Sons; 2011. DOI: 10.1002/978047082 8847. ch12. ISBN 978-0-470-82882-3

[18] Kallio M, Vuorinen P, Fuentes E, Maraña O, Ruusila V, Nyysönnen T, et al. Tribological behaviour of bronze alloys with solid lubricants. Key Engineering Materials. 2013;**527**:205-210

[19] Igartua A, Laucirica J, Aranzabe A. Application of low temperature PVD coatings in rolling bearings. Tribological tests and experiences with spindle bearing systems. Surface and Coating Technology. 1996;**1**:460-467. DOI: 10.1016/ S0257-8972(96)03050-2

[20] Zabala B. Doctoral thesis. Universidad País Vasco; 2017

10.1016/j.surfcoat.2018.06.089

[16] López-Ortega A, Arana JL, Rodríguez E, Bayón R. Corrosion, wear and tribocorrosion performance of a thermally sprayed aluminum coating modified by plasma electrolytic oxidation for offshore submerged components protection. Corrosion Science. 2018;**143**:258-280. DOI: 10.1016/j.corsci.2018.08.001

**174**

[30] Sáenz de Viteri V, Fuentes E. Titanium and Titanium Alloys as Biomaterials. Rijeka, Croatia: InTech. DOI: 10.5772/55860

[31] Sáenz de Viteri V, Bayon R, Igartua A, Barandika G, Moreno JE, Pérez C, et al. Structure, tribocorrosion and biocide characterization of Ca, P and I containing TiO2 coatings developed by plasma electrolytic oxidation. Applied Surface Science. 2016;**367**:1-10. DOI: 10.1016/j.apsusc.2016.01.145

[32] Igartua A, Bayon R, Mendoza G. Plasma electrolytic oxidation coatings for engine components. Ricerca e Sviluppo. 2014;**67**:44-52

[33] Laucirica J, Arnaiz A, Igartua A. Mantenimiento y control mediante Sistema experto; Forum Calidad. Vol. 361992. pp. 54-61

[34] Presa J, Fernández-Díaz B, Igartua A, San José E, Almandoz X, Rodríguez JC, et al. Effects of manufacturing errors in the behaviour of a power gearbox. In: LUBMAT Conference; June 2016. 2016. Available from: https:// www.slideshare.net/TogetherToSolve/ effects-of-manufacturing-errors-in-thebehaviour-of-a-power-gearbox

[35] Martins R, Seabra J, Brito A, Seyfert C, Luther R, Igartua A. Friction coefficient in FZG gears lubricated with industrial gear oils: Biodegradable ester vs. mineral oil. Tribology International. 2006;**39**:512-521. DOI: 10.1016/j. triboint.2005.03.021

[36] Cardoso NFR, Martins RC, Seabra JHO, Igartua A, Rodriguez JC, Luther R. Micropitting performance of nitrided steel gears lubricated with mineral and ester oils. Tribology International.

2008;**42**(1):77-87. DOI: 10.1016/j. triboint. 2008.05.010

[37] Martins RC, Cardoso NFR, Bock H, Igartua A, Seabra JHO. Power loss performance of high pressure nitrided steel gears. Tribology International. 2009;**42**:1807-1815. DOI: 10.1016/j. triboint.2009.03.006

[38] Leao JD, Bouillon V, Muntada L, Johnson C, Wilson P, Vergnes O, et al. New formulations of sunflower based bio-lubricants with high oleic acid content. Oilseeds and fats, Crops and Lipids. 2016;**23**(5):D509. DOI: 10.1051/ ocl/2016033

[39] Igartua A, Barriga J, Aranzabe A. Biodegradable Lubricants. Vol. 1. Radom, Poland: Virtual Tribological Institute; 2005. pp. I.1-VI.3. ISBN 83-7204-449-X

[40] Vercammen K, Van Acker K, Barriga J, Fuentes E, Kalin M, Vizintin J. Combining biolubricants and low friction coatings. In: Current Trends in Tribology. Vol. I. Poland: ITEE; 2005. pp. 1-4. ISBN 83-70204-418-X

[41] Igartua A. Biolubricants & their control for sustainable developments. Lube. 2007;**81**:6. ISSN 1744-5418

[42] Zabala B, Igartua A, Scarpi V, Timelli G, Girot F. Multiparametric study of Leidenfrost point and wettability of lubricants on highpressure die-casting dies. International Journal of Thermal Sciences. 2018;**125**:66-73. DOI: 10.1016/j. ijthermalsci.2017.11.014

[43] Zabala B, Igartua A, Raone C, Timelli G, Bonollo F, Scarpi V, Peggiato M, Girot F, "Evaluation HPDC Lubricant Spraying for Improved Cooling and Die Protection, LUBMAT Conference, 2016. Available from: https://www.researchgate.net/ publication/315837772\_Evaluation\_ HPDC\_Lubricant\_Spraying\_for\_ Improved\_Cooling\_and\_Die\_Protection [44] Barriga J, Igartua A, Marín M. Mejora del proceso de forja mediante la aplicación de nitruración a alta presión y la introducción de una lubricación ecológica. Boletin de la Sociedad Espanola de Ceramica y Vidrio. 2004;**13**(2). DOI: 10.3989/cyv.2004.v43. i2.491

[45] Caliari D, Timelli G, Igartua A. Microstructural and tribological investigations of diecast and hard anodized AlSiCu alloys. Surface and Coatings Technology. 2018;**352**:462-273. DOI: 10.1016/j.surfcoat.2018.07.084

[46] Zabala B, Igartua A, Fernandez X, Nevshupa R. Friction and wear of a piston ring/cylinder liner at the top dead center: Experimental study and modelling. Tribology International. 2017;**106**:23-33. DOI: 10.1016/j. triboint.2016.10.005

[47] Igartua A, Fernandez X, Woydt M, Luther R, Illarramendi I. Tribological tests to simulate wear in piston rings. In: Critical Component Wear in Heavy Duty Engines. Vol. 1. 2011. pp. 167-195. DOI: 10.1002/9780470828847.ch11

[48] Igartua A, Fernández X, Areitioaurtena O, Luther R, Seyfert C, Rausch J, et al. Biolubricants and triboreactive materials for automotive applications. Tribology International. 2009;**42**:561-568. DOI: 10.1016/j. triboint.2008.10.015

[49] Picas JA, Forn A, Igartua A, Mendoza G. Mechanical and tribological properties of high velocity oxy-fuel thermal sprayed nanocrystalline CrC-NiCr coatings. Surface and Coating Technology. 2013;**174-175**:1095-1100. DOI: 10.1016/S0257-8972(03)00393-1

[50] Bellido-González V, Igartua A, Mendoza G, Powell S, Talks MG, Momeñe E. Replacement of hardchrome in cylinder liners. A PVD approach. Society of Vacuum Coaters. 2004:505-856. ISBN 0737-5921

[51] Igartua A, Tonder K. COST 532-Triboscience and tribotechnology superior friction and wear control in engines and transmissions. In: Engine Systems. Belgium: COST Edition; 2008. pp. 108-113. ISBN: 978-92-898-0040-2

[52] Fdez-Pérez X, Igartua A, Nevshupa R, Zabala P, Zabala B, Luther R, et al. Innovative "green" tribological solutions for clean small engines. In: Gegner J, editor. Tribology-Fundamentals and Advancements. Rijeka, Croatia: IntechOpen; DOI: 10.5772/55836. Available from: https://www. intechopen.com/books/tribologyfundamentals-and-advancements/ innovative-green-tribological-solutionsfor-clean-small-engines

[53] Gili F, Igartua A, Luther R, Woydt M. The impact of biofuels on engine oil performance. Lubrication Science. 2011;**23**(7):313-330. DOI: 10.1002/ls.158

[54] Igartua A, Nevshupa R, Fernandez X, Conte M, Zabala R, Zabala P, et al. Alternative eco-friendly lubes for clean two-stroke engines. Tribology International. 2011;**44**:727-736. DOI: 10.1016/j.triboint.2010.01.019

[55] Available from: http://slipsafe.org/

[56] Igartua A, Saenz de Viteri V, Fuentes E. Tribological response of the cotton textile against human skin equivalents. In: The International Istambul Textile Congress. 30th May-1st June 2013

[57] Fuentes E, Sáenz de Viteri V, Igartua A, Martinetti R, Dolcini L, Barandika G. Structural characterization and mechanical performance of Ca/P scaffolds and natural bones: A comparative study. Journal of Applied Biomaterials & Biomechanics. 2010;**8**:159-165. DOI: 10.5301/ JABB.2010.6092

[58] Alves SA, Bayon R, Igartua A, Saenz de Viteri V, Rocha A. Tribocorrosion behavior of anodic titanium oxide

**177**

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process*

Journal of Engineering Tribology.

[66] Kronberger M, Pagano F, Pejakovic V, Igartua A, Urbistondo E, Kalin M. Miscibility and tribological investigation of ionic liquids in biodegradable esters. Lubrication Science. 2014;**26**:463-387. DOI: 10.1002/

[67] Stolte S, Steudte S, Areitioaurtena O, Pagano F, Thöming J, Stepnowski P, et al. Ionic liquids as lubricants or lubrication additives: An ecotoxicity and biodegradability assessment. Chemosphere. 2012;**89**:1135-1141. DOI: 10.1016/j.chemosphere.2012.05.102

[68] Gilabert E, Gorritxategi E, Conde E, Garcia A, Areitioaurtena

maintenance system for polygeneration applications. In: Engineering Asset Lifecycle Management. 2010. pp. 823-830. Available from: https:// rd.springer.com/chapter/10.1007 %2F978-0-85729-320-6\_94

[69] Holmberg K, Erdermir A. Influence

[70] Igartua A, Urdangarín L, Pérez de Larraya D. Motores de barco adaptados al uso de lubricantes y fueles alternativos, Europa Azul. 2008.

[71] Cerrillo C, Barandika G, Igartua A, Areitioaurtena O, Mendoza G. Key challenges for nanotechnology: Standardization of ecotoxicity testing. Journal of Environmental Science and Health, Part C. 2016;**4**:89-104. https://

[72] Cerrillo C, Barandika G, Igartua A, Areitioaurtena A, Uranga N, Mendoza G. Colloidal stability and ecotoxicity of multiwalled carbon

doi.org/10.1002/etc.2999

of tribology on global energy consumption, costs and emissions. Friction. 2017;**5**(3):263-284. DOI: 10.1007/ s40544-017-0183-5

pp. 68-69

O, Igartua A. An advanced

2012;**117**:359-366

ls.1274

*DOI: http://dx.doi.org/10.5772/intechopen.85616*

films produced by plasma electrolytic

Lubrication Science. 2014;**26**:500-513.

[59] (a) Zhang S, Zeng X, Matthews DTA, Igartua A, Rodriguez-Vidal E, Contreras Fortes J, et al. Selection of micro-fabrication techniques on stainless steel sheet for skin friction. Friction. 2016;**4**:89-104. DOI: 10.1007/ s40544-016-0115-9. (b) Rodriguez E, Igartua A. Texture design for reducing tactile friction independent of sliding orientation on stainless steel sheet. Tribology Letters. 2017;**3**:65-89. DOI:

oxidation for dental implants.

10.1007/s11249-017-0869-x

[60] Mendoza G, Igartua A, Arizaga I, Azpiazu F, Santiso G. Metal working fluids based on vegetable oils for grinding operations. Journal of Mechanics Engineering and Automation. 2012;**2**(10):638-646

[61] Igartua A, Barriga J, Pérez J, Muntada L, Navío P. Ecological lubricants for cutting and forming applications. In: New Horizons for Tribology and Lubricants; Expert Verlag 2002. Vol. 10. Austria: OETG; 2001. pp. 60-64. Available from: http://www. oetg.at/fileadmin/Dokumente/oetg/ Proceedings/WTC\_2001\_files/html/M-

29-13-751-IGARTUA.pdf

[62] Igartua A. Biodegradable lubricants. Lube. 2007;**82**:19-22. ISSN 1744-5418

[63] Igartua A, Mendoza G, Fernandez-

Arguizoniz R. Vegetable oils as hydraulic fluids for agricultural applications. Grasas y Aceites. 2011;**62**:29-38. DOI: 10.3989/gya.056210. ISBN: 0017-3495

[64] Igartua A Synthetic lubrication and tribotest. Lubrication Science. 2014;**26**:447-448. DOI: 10.1002/ls.1277

[65] Pagano F, Zare P, Mahrova M, Dörr N, Bayon R, Fernandez X, et al. Dicationic ionic liquids as lubricants.

Diaz B, Urquiola F, Vivanco S,

DOI: 10.1002/ls.1234

*Tribology: The Tool to Design Materials for Energy-Efficient and Durable Products and Process DOI: http://dx.doi.org/10.5772/intechopen.85616*

films produced by plasma electrolytic oxidation for dental implants. Lubrication Science. 2014;**26**:500-513. DOI: 10.1002/ls.1234

*Friction, Lubrication and Wear*

i2.491

[44] Barriga J, Igartua A, Marín M. Mejora del proceso de forja mediante la aplicación de nitruración a alta presión y la introducción de una lubricación ecológica. Boletin de la Sociedad Espanola de Ceramica y Vidrio.

[51] Igartua A, Tonder K. COST 532-Triboscience and tribotechnology superior friction and wear control in engines and transmissions. In: Engine Systems. Belgium: COST Edition; 2008. pp. 108-113. ISBN: 978-92-898-0040-2

for-clean-small-engines

[52] Fdez-Pérez X, Igartua A, Nevshupa R, Zabala P, Zabala B, Luther R, et al. Innovative "green" tribological solutions for clean small engines. In: Gegner J, editor. Tribology-Fundamentals and Advancements. Rijeka, Croatia: IntechOpen; DOI: 10.5772/55836. Available from: https://www. intechopen.com/books/tribologyfundamentals-and-advancements/ innovative-green-tribological-solutions-

[53] Gili F, Igartua A, Luther R, Woydt M. The impact of biofuels on engine oil performance. Lubrication Science. 2011;**23**(7):313-330. DOI: 10.1002/ls.158

[54] Igartua A, Nevshupa R, Fernandez X, Conte M, Zabala R, Zabala P, et al. Alternative eco-friendly lubes for clean two-stroke engines. Tribology International. 2011;**44**:727-736. DOI: 10.1016/j.triboint.2010.01.019

[55] Available from: http://slipsafe.org/

[56] Igartua A, Saenz de Viteri V, Fuentes E. Tribological response of the cotton textile against human skin equivalents. In: The International Istambul Textile Congress. 30th May-1st June 2013

[57] Fuentes E, Sáenz de Viteri V, Igartua A, Martinetti R, Dolcini L, Barandika G. Structural characterization and mechanical performance of Ca/P scaffolds and natural bones: A

comparative study. Journal of Applied

[58] Alves SA, Bayon R, Igartua A, Saenz de Viteri V, Rocha A. Tribocorrosion behavior of anodic titanium oxide

Biomaterials & Biomechanics. 2010;**8**:159-165. DOI: 10.5301/

JABB.2010.6092

2004;**13**(2). DOI: 10.3989/cyv.2004.v43.

[45] Caliari D, Timelli G, Igartua A. Microstructural and tribological investigations of diecast and hard anodized AlSiCu alloys. Surface and Coatings Technology. 2018;**352**:462-273. DOI: 10.1016/j.surfcoat.2018.07.084

[46] Zabala B, Igartua A, Fernandez X, Nevshupa R. Friction and wear of a piston ring/cylinder liner at the top dead center: Experimental study and modelling. Tribology International. 2017;**106**:23-33. DOI: 10.1016/j.

[47] Igartua A, Fernandez X, Woydt M, Luther R, Illarramendi I. Tribological tests to simulate wear in piston rings. In: Critical Component Wear in Heavy Duty Engines. Vol. 1. 2011. pp. 167-195. DOI: 10.1002/9780470828847.ch11

[48] Igartua A, Fernández X, Areitioaurtena O, Luther R, Seyfert C, Rausch J, et al. Biolubricants and triboreactive materials for automotive applications. Tribology International. 2009;**42**:561-568. DOI: 10.1016/j.

[49] Picas JA, Forn A, Igartua A,

[50] Bellido-González V, Igartua A, Mendoza G, Powell S, Talks MG, Momeñe E. Replacement of hardchrome in cylinder liners. A PVD approach. Society of Vacuum Coaters.

2004:505-856. ISBN 0737-5921

Mendoza G. Mechanical and tribological properties of high velocity oxy-fuel thermal sprayed nanocrystalline CrC-NiCr coatings. Surface and Coating Technology. 2013;**174-175**:1095-1100. DOI: 10.1016/S0257-8972(03)00393-1

triboint.2008.10.015

triboint.2016.10.005

**176**

[59] (a) Zhang S, Zeng X, Matthews DTA, Igartua A, Rodriguez-Vidal E, Contreras Fortes J, et al. Selection of micro-fabrication techniques on stainless steel sheet for skin friction. Friction. 2016;**4**:89-104. DOI: 10.1007/ s40544-016-0115-9. (b) Rodriguez E, Igartua A. Texture design for reducing tactile friction independent of sliding orientation on stainless steel sheet. Tribology Letters. 2017;**3**:65-89. DOI: 10.1007/s11249-017-0869-x

[60] Mendoza G, Igartua A, Arizaga I, Azpiazu F, Santiso G. Metal working fluids based on vegetable oils for grinding operations. Journal of Mechanics Engineering and Automation. 2012;**2**(10):638-646

[61] Igartua A, Barriga J, Pérez J, Muntada L, Navío P. Ecological lubricants for cutting and forming applications. In: New Horizons for Tribology and Lubricants; Expert Verlag 2002. Vol. 10. Austria: OETG; 2001. pp. 60-64. Available from: http://www. oetg.at/fileadmin/Dokumente/oetg/ Proceedings/WTC\_2001\_files/html/M-29-13-751-IGARTUA.pdf

[62] Igartua A. Biodegradable lubricants. Lube. 2007;**82**:19-22. ISSN 1744-5418

[63] Igartua A, Mendoza G, Fernandez-Diaz B, Urquiola F, Vivanco S, Arguizoniz R. Vegetable oils as hydraulic fluids for agricultural applications. Grasas y Aceites. 2011;**62**:29-38. DOI: 10.3989/gya.056210. ISBN: 0017-3495

[64] Igartua A Synthetic lubrication and tribotest. Lubrication Science. 2014;**26**:447-448. DOI: 10.1002/ls.1277

[65] Pagano F, Zare P, Mahrova M, Dörr N, Bayon R, Fernandez X, et al. Dicationic ionic liquids as lubricants. Journal of Engineering Tribology. 2012;**117**:359-366

[66] Kronberger M, Pagano F, Pejakovic V, Igartua A, Urbistondo E, Kalin M. Miscibility and tribological investigation of ionic liquids in biodegradable esters. Lubrication Science. 2014;**26**:463-387. DOI: 10.1002/ ls.1274

[67] Stolte S, Steudte S, Areitioaurtena O, Pagano F, Thöming J, Stepnowski P, et al. Ionic liquids as lubricants or lubrication additives: An ecotoxicity and biodegradability assessment. Chemosphere. 2012;**89**:1135-1141. DOI: 10.1016/j.chemosphere.2012.05.102

[68] Gilabert E, Gorritxategi E, Conde E, Garcia A, Areitioaurtena O, Igartua A. An advanced maintenance system for polygeneration applications. In: Engineering Asset Lifecycle Management. 2010. pp. 823-830. Available from: https:// rd.springer.com/chapter/10.1007 %2F978-0-85729-320-6\_94

[69] Holmberg K, Erdermir A. Influence of tribology on global energy consumption, costs and emissions. Friction. 2017;**5**(3):263-284. DOI: 10.1007/ s40544-017-0183-5

[70] Igartua A, Urdangarín L, Pérez de Larraya D. Motores de barco adaptados al uso de lubricantes y fueles alternativos, Europa Azul. 2008. pp. 68-69

[71] Cerrillo C, Barandika G, Igartua A, Areitioaurtena O, Mendoza G. Key challenges for nanotechnology: Standardization of ecotoxicity testing. Journal of Environmental Science and Health, Part C. 2016;**4**:89-104. https:// doi.org/10.1002/etc.2999

[72] Cerrillo C, Barandika G, Igartua A, Areitioaurtena A, Uranga N, Mendoza G. Colloidal stability and ecotoxicity of multiwalled carbon

nanotubes: influence of select organic matters. Environmental Toxicology and Chemistry. 2016;**35**:74-83. https://doi. org/10.1002/etc.3172

[73] Cerrillo C, Barandika G, Igartua A, Areitioaurtena O, Mendoza G. Towards the standardization of nanoecotoxicity testing: Natural organic matter 'camouflages' the adverse effects of TiO2 and CeO2 nanoparticles on green microalgae. Science of the Total Environment. 2016;**543**(A1):95- 104. https://doi.org/10.1016/j. scitotenv.2015.10.137

[74] Laux P, Riebeling C, Booth AM, Brain JD, Brunner J, Cerrillo C. Challenges in characterizing the environmental fate and effects of carbon nanotubes and inorganic nanomaterials in aquatic systems. Environmental Science: Nano. 2018;**5**:48-63. DOI: 10.1039/C7EN00594F

[75] Laux P, Riebeling C, Booth AM, Brain JD, Brunner J, Cerrillo. Biokinetics of Nanomaterials: the Role of Biopersistence. NanoImpact. 2017;**6**:69-80. DOI: 10.1016/j. impact.2017.03.003

**179**

**films**

**Chapter 10**

*Hongbo Ju*

**Abstract**

metal nitride film are also discussed.

**1. Introduction**

High-Temperature Self-

Lubricating Metal Nitride-Based

Nanostructure Composite Films

The film technology is one of the most efficient methods of modifying the surface properties of materials. The focus of recent attention in the solid lubricating materials is on the hard transition metal nitride films' excellent high-temperature tribological properties applied in powertrains and cutting tools. This chapter reviewed the formation mechanism of Magnéli phases and the influence of Magnéli phases on the high-temperature tribological properties of hard transition metal nitride films synthesized using magnetron sputtering. The self-lubricating behavior and wear mechanism of the Magnéli phases are discussed from the point of view of crystallography. Some methods to enhance the wear resistance property of the

Recently, a solid lubrication known as Magnéli phases was reported in the application of oxide materials with "easy" crystallographic shear phases, and numerous related research activities have been carried out to investigate the function mechanism of Magnéli phases. Molybdenum, tungsten, and vanadium as the additional elements were initially incorporated into transition metal nitride (TMN)-based hard films, since the molybdenum oxide, tungsten oxide, and vanadium oxide are common Magnéli phases and exhibit the excellent lubricating property. The TMN matrix as the hard phase with a columnar structure could retain the strength and bearing capacity during the wear test. Both the environment heat and friction heat induce the complex tribo-chemistry reaction and the formation of Magnéli phases. The binary molybdenum nitride, the scientists have already attached importance to tungsten nitride and vanadium nitride film in solid lubricating films in recent years. In this part, the high-temperature self-lubricating property of TMN-based hard films was discussed.

**2. Binary molybdenum nitride, tungsten nitride, and vanadium nitride** 

The crystal structure of the molybdenum nitride film shows a little influence on the deposition parameters such as nitrogen partial pressure, substrate temperature,

**Keywords:** transition metal nitride films, magnetron sputtering,

tribological properties, self-lubricating, Magnéli phase

### **Chapter 10**

*Friction, Lubrication and Wear*

org/10.1002/etc.3172

nanotubes: influence of select organic matters. Environmental Toxicology and Chemistry. 2016;**35**:74-83. https://doi.

[73] Cerrillo C, Barandika G, Igartua A, Areitioaurtena O, Mendoza G. Towards the standardization of

matter 'camouflages' the adverse effects of TiO2 and CeO2 nanoparticles on green microalgae. Science of the Total Environment. 2016;**543**(A1):95-

104. https://doi.org/10.1016/j.

[74] Laux P, Riebeling C, Booth AM, Brain JD, Brunner J, Cerrillo C. Challenges in characterizing the

[75] Laux P, Riebeling C, Booth AM, Brain JD, Brunner J, Cerrillo. Biokinetics of Nanomaterials: the Role of Biopersistence. NanoImpact.

2017;**6**:69-80. DOI: 10.1016/j.

environmental fate and effects of carbon nanotubes and inorganic nanomaterials in aquatic systems. Environmental Science: Nano. 2018;**5**:48-63. DOI:

scitotenv.2015.10.137

10.1039/C7EN00594F

impact.2017.03.003

nanoecotoxicity testing: Natural organic

**178**
